1. FibreAny raw material that has hair like appearance or has a tapered elongated shapeis called as a fibre. The fibre has a length that is at least one thousand timesthan its thickness. This high ratio of length to its thickness is responsible for itspeculiar hair like appearance.Fibres occur naturally or they can be artificially produced by using chemicals. Notall the fibres are suitable for the production of textile goods i.e. yarns andfabrics.Textile FibreA textile fibre is the basic unit of raw material for making a yarn. The textilefibres must have a suitable length, pliability, fineness and strength that isnecessary for their conversion into yarns and fabrics. A fibre having an extremelength is called as a filament.YarnYarn is a continuous strand composed of either natural or manmade fibres orfilaments and is used in weaving and knitting to produce a cloth. ORA yarn is defined as a product of substantial length and relatively small cross-section consisting of fibres and / or filament(s) with or without twist. (Textile Institute)SpinningSpinning may be defined as the process of converting fibres and / or filament(s)into a yarn.In the production of manmade fibres, the extrusion of the fibre forming liquidthrough the spinnerets followed by hardening of these liquid jets into solidfilaments is called as the process of spinning.The meaning of the term spinning in this case may be completely different fromthat used for natural fibres. Generally we can define spinning as a process thatproduces a yarn as its final product. The spinning of manmade fibres can becarried out by three different methods:(i) Wet Spinning.(ii) Dry Spinning.(iii) Melt Spinning.These different types of spinning methods are used based on the properties ofthe fibre forming substance. For example in order to spin Viscose Rayon, wetspinning is used and for Nylon we use the melt spinning. Some fibre formingsubstances can be spun by using more than one type of the above mentionedspinning techniques.
2. The Making of a Textile Product
3. Yarn ClassificationThere is no limit of the range of yarns that can be produced by various types ofspinning processes. So it is difficult to classify various types of yarns on a singlebasis. Yarns can be classified on various grounds.
4. Fibre Properties That Can Influence SpinningIn general there are numerous fibre properties that are important to consider asthese properties have a large influence on the final end product produced fromit. It is also important to know every detailed fibre property because it helps usto decide the type processes that should be used for a particular fibre. Howeverstrictly speaking from spinning viewpoint the most important fibre propertiesthat determine the spinning ability are:(1) Fibre Staple Length(2) Fibre Fineness(3) Fibre Strength(1) Fibre Staple LengthLength of the fibre is the most important property that determines the qualityand value of the fibre and it also determines its spinning ability. Most naturalfibres have a length ranging from ¼” to about 3”. But the silk fibre made bysilkworm is in a continuous filament form that can have a length of up to 2kilometres. Apart from silk the all the natural fibres are valued from their staplelength, greater the staple length greater will be their value. The staple length ofthe natural fibres obtained from a same source can vary. So the actual staplelength given to the fibre is the length of the majority of the fibres in a lot.On the other hand the synthetic fibres can have unlimited length in a filamentform or they can be cut into a desired staple length. This is true because theyare produced chemically in laboratories. Synthetic fibres either in filament orstaple form will have perfect uniformity of length among themselves.Staple length of fibres play important role in their conversion to a yarn. Ingeneral the longer the individual fibres easier it is to convert them to yarn due tothe fact that long fibres will have to overlap at less frequent points as comparedto short fibres and that is the reason that longer fibres can easily be spun into ayarn with less twist. Furthermore it takes less twist to convert long fibres into ayarn as compared to short fibres.
5. (2) Fibre FinenessThe fineness of the fibre is also an important parameter that controls spinningability of the fibres to be converted into a yarn. Finer the individual fibres are,the finer the yarn can be made out of it. A yarn spun with finer fibres will havemore number of fibres per unit cross-section as compared to a yarn havingcoarse fibres. This considerably increases the cohesion among the fibres withinthe yarn. Also the fine fibres tend to be more flexible and pliable than the coarseones, which enables them to be spun more effectively into a yarn.The measure of fineness of the fibres that is how thick or thin they are, isexpressed in terms of fibre count. The direct method of measuring fineness orthe count of the fibre is to express the thickness or diameter of the fibre interms of microns, where 1 micron = 0.001 mm.More practically, the count of the fibre is expressed in terms of mass per unitlength i.e. the linear density. The linear density is expressed in terms ofmilligrams per kilometer (millitex unit), grams per kilometer (Tex unit), gramsper 9000 metres (denier unit). Sometimes the mass per unit length is alsoexpressed in grams per centimeter (usually in 10-8 grams / cm).(3) Tensile StrengthThe tensile strength of a textile fibre is the ability of a fibre to resist a stretchingload when applied in the longitudinal direction. Whenever a pulling or astretching load is applied to a textile fibre, it starts elongating. As the loadapplied to it gradually increases, a point comes when the fibre is no longer ableto resist that load and it breaks. In this way the tensile strength of a fibre isfound out. The tensile strength of a fibre is also called as the breaking load i.e.the load under which the fibre breaks.In case of a single fibre, the strength of the fibre is better expressed in terms oftenacity. Tenacity can be defined as the ratio of the breaking load to the massper unit length and is also a measure of specific stress at break. Tenacity = Breaking Load / Mass per unit lengthTenacity is usually expressed in grams per tex, grams per decitex, grams perdenier, centiNewton per Tex (cN/Tex).It may be noted that two fibres with the same tenacity can have different tensilestrength depending upon their densities or cross-section area.The maximum achievable strength of the yarn is dependent upon the strength ofindividual fibres.
6. Yarn DimensionsThere are number of parameters that can describe a yarn, however following arethe most important yarn properties:(1) Yarn Count(2) Yarn Twist(3) Yarn Strength(1) Yarn CountThe yarn count or the yarn number is the relationship between the mass and thelength of the yarn. Yarn count or yarn number actually describes the lineardensity of a yarn i.e. mass per unit length. In simpler words, the yarn number isthe measure of thickness of yarn. There are two types of yarn numberingsystems :- (i) Indirect System (ii) Direct System(i) Indirect SystemThe indirect counting system is also known as the English counting system. It isan old system of yarn counting or numbering and is only used for natural fibreslike cotton, jute, wool, flax, etc.This system is called as indirect because here the yarn count has an indirectrelationship with its weight. Which means that as the count increases, the yarnbecomes finer. In this system, the weight is kept constant while the length is variable and thenumber of hanks that weighs a unit weight gives the indirect count. Indirect Count = Length / WeightThe most commonly used Indirect numbering systems are :- (a) Cotton System (b) Metric System or Continental System(a) Cotton SystemThe Cotton count may be defined as the number of hanks per pound. Where onehank is a specific length of a yarn, for cotton fibres, it is 840 yards. Cotton Count = Number of Hanks / 1 PoundAlthough this Counting system can be used for many natural fibres, but still it isknown as cotton system because it is mostly used for cotton fibres.
7. The hank length for different fibres is different depending upon the nature of thefibre. Different hank lengths for different fibres are given below :- Nature of Fibre Hank Length Cotton 840 Yards Spun Silk 840 Yards Wool 256 Yards Worsted 560 Yards Linen 300 Yards Jute 14400 Yards(b) Metric System or Continental SystemThe Continental system is similar to cotton system and can be defined as thenumber of hanks per kilogram. Here the hank length is fixed at 1000 metres. Continental Count = Number of Hanks / 1 KG(ii) Direct SystemThe direct numbering system is also called as French numbering system. It is amodern counting system which can be used for both natural and manmadefibres. This system is called as the direct system because here the yarn counthas a direct relationship with its weight and is given by :- Direct Count = Weight / LengthIn the direct system, the length is kept constant, while the weight varies. Sincethe yarn has a direct relationship with its weight therefore, as the countincreases, the yarn becomes coarser.There are many direct numbering systems, the most widely used are :- (a)Denier (b)Tex (c)Grex(a) DenierDenier count is the number of grams per 9000 metres of a yarn. Denier Count = Number of Grams / 9000 MetresIt means that the weight of 9000 metres of yarn gives the Denier count.(b) TexTex count is the number of grams per 1000 metres of a yarn. Tex Count = Number of Grams / 1000 MetresIt means that the weight of 1000 metres of yarn gives the Tex count.
8. (c) GrexGrex count is the number of grams per 10,000 metres of a yarn. Grex Count = Number of Grams / 10,000 MetresIt means that the weight of 10,000 metres of yarn gives the Grex count.Conversion FactorThe indirect or English number can be converted into direct or French number byusing the following relations :- (1) Cotton Count x Tex Count = 590.5 (2) Cotton Count x Grex Count = 5905 (3) Cotton Count x Denier Count = 5315 (4) Denier Count = 9 x Tex Count(2) Yarn TwistThe short staple fibres are always twisted together during the process ofspinning to produce a yarn. The twist is actually given to bind the fibres togetheras a yarn and to give yarn strength. The amount of twist not only directly affectsthe strength of the yarn; it also affects lustre, abrasion resistance, handle,absorbency and flexibility.The twist during spinning is inserted by rotating the fibre strand in eitherclockwise or counter clockwise direction. The direction of the twist is defined byusing the letters ‘S’ and ‘Z’. The ‘S’ twisted yarn is the one in which the directionof the twist or the spiral of the yarn is parallel to the centre bar of the letter ‘S’.Similarly the ‘Z’ twisted yarn has its twist direction parallel to the centre bar ofthe letter ‘Z’. A spindle rotating counter clockwise will produce ‘S’ twist while thespindle rotating clockwise will result in ‘Z’ twist. S-Twisted Yarn Z-Twisted YarnThe direction of the twist is very important in folded and cabled yarn where thedirection of the twist of the individual thread and the direction of twist of foldingand cabling affects the properties of the resultant yarn. The direction of twist ofthe yarn can also affect some woven fabric structures like twill weaves.The majority of the cotton spun yarns are ‘Z’ twisted this is due to the fact thatmost of the spinning equipment are designed for producing ‘Z’ twisted yarnsbecause such an equipment will favour a right-handed person as he does thenecessary repairing and maintenance of machine parts.
9. The amount of twist in a yarn is expressed in terms of turns per unit lengthusually in turns per inch (tpi), turns per centimetre and turns per meter. Theyarn with a low twist will be weaker, softer and bulkier. In general to hold and togive strength to short fibres more twist is required.As the degree of twist in a yarn increases the strength of the yarn alsoincreases. However when the amount of twist is further increased beyond anoptimum value then on further increase of twist, the strength of the yarndecreases. This is due to the fact that with an excessive twist, the fibres tend tobe more perpendicular than parallel to the length of the yarn i.e. they loose theirlinear orientation and also because with an excessive twist fibre breakageoccurs.Assuming the yarn as a perfect cylinder, consider a yarn having a length (l) anddiameter (d) with only one turn of twist inserted into it. If the yarn is cut fromthe centre and is laid flat then it would look like a rectangle as shown below:It is very important to establish a relationship between the helix angle (θ) andthe tpi inserted in a yarn. The helix angle (θ) depends upon the amount of twistpresent in a yarn. With a change in the value of tpi, the helix angle (θ) will alsochange.From the above figure: Tan θ = πd / lBut l = 1 / tpi and d = 1 28 NcSo π x tp i Tan θ = 28 NcThis equation shows that the helix angle (θ) is also related to the count of theyarn. If the helix angle (θ) is to be kept constant, the ratio of tpi and yarn countshould also be kept constant. In other words to spin yarns of various differentcounts but with the same twist characteristics this ratio should remain the same.
10. Which means that twist or tpi in a yarn is directly related to the fineness orcount of the yarn. Fine yarns would usually require a higher value of tpi thancoarse ones.To calculate the amount of optimum tpi required for various counts of yarns aterm called as twist multiplier comes into play. Twist multiplier (TM) is definedas the ratio of the tpi to the square root of the cotton count. tp i T w is t M u lt ip lie r = T M = NcDifferent types of yarns according to the end usage are spun with differentvalues of TM. For example knitted yarns or hosiery yarns are spun with a TM of 2to 3, weaving yarns with a TM of 3 to 5 and hard twisted crepe yarns are twistedwith up to a TM of 7. Too much twist makes the yarn hard, brittle and causesnarls in the yarn and becomes hard to knit and weave.(3) Yarn StrengthAll the staple yarns consist of fibres twisted together. The purpose of twisting isto bind the fibres together so as to strengthen the yarn. If a load is applied to ayarn with a low twist then that yarn may break easily. This breakage may not bedue to the breakage of fibres but because of the slippage of the fibres. As theamount of twist increases, the level of cohesiveness among the fibres will alsoincrease making the yarn stronger and more compact. Such a yarn wouldrequire a bigger load to break it.So the major source of strength to the yarn is provided by the twist. As the twistincreases, the strength of the yarn also increases. However this is only true upto a certain limit of twist called as the optimum twist. Beyond the optimum twist,on further increase in twist will reduce the strength of the yarn. This is becauseof the two factors:(i) Excessive twist causes obliquity in the fibres and the fibres tend to lie more perpendicular than parallel to the length of the yarn i.e. they loose their linear orientation.(ii) Secondly with an excessive twist fibre breakage occurs.The relationship between the yarn strength and the twist is shown by thefollowing graph:
11. Folded & Cabled YarnsFolded YarnsFolded or plied yarns are spun from two or more single yarns by twisting themtogether. Two fold or two ply yarn for example is composed of two single yarnsand three ply or three fold yarn is composed of three single yarns. Dependingupon twist direction two methods are used to make a plied yarn:(i) All the individual single yarns are twisted in one direction and are then combined and twisted in the opposite direction to form a uniform and soft folded or plied yarn.(ii) All the individual single yarns are twisted in one direction and are again combined and twisted in the same direction to form a hard and less flexible folded or plied yarn.Uses of Folded Yarns(i) Folded yarns are used for heavy industrial fabrics where extra strength is needed.(ii) By the process of folding, a very coarse yarn that is impossible to make on ordinary spinning machines can be made.(iii) Folded yarns made from very fine fibres are used in delicate looking sheer fabrics.Cabled YarnsCabled or Corded yarns are produced by twisting two or more plied or foldedyarns together.
12. Cabled or Corded yarns can be produced by different combinations of twistdirections:(i) Usually cabled yarns are made with the final twist usually applied in the opposite direction of the ply twist.(ii) Cables or cords may follow an SZS form, with S-twisted singles made into Z-twisted plies that are then combined with an S-twist, or may follow a ZSZ form.(iii) Cabled or corded yarn may also follow an SSZ or a ZZS pattern.Uses of Cabled or Corded Yarns(i) Corded yarns may be used as rope or twine.(ii) They may also be made into very heavy industrial fabrics(iii) Cables made from extremely fine fibres are used to make sheer dress fabrics.Count of Folded and Cabled YarnsIn order to find out the count of the folded and cabled yarns we use thefollowing formula :-For Direct Numbering system :- Final Count = C1 + C2 + C3 + C4 + ………………………..Where, C1, C2, C3, C4, ……….. are the counts of the threads out of which thefolded yarn or cabled yarn is made.For Indirect numbering system :- 1/Final Count = 1/C1 + 1/ C2 + 1/ C3 + 1/ C4 + …………………………Where, C1, C2, C3, C4, ……….. are the counts of the threads out of which thefolded yarn or cabled yarn is made.For using these formulas, the count system of each yarn in the folded or cabledyarns must be the same.
13. Variables in Yarn ProductionMost generally yarns can be classified into continuous filament yarns made outof manmade raw material and short staple yarns produced from natural fibres.However within these two categories endless varieties of yarns can be producedbecause there are so many variables involved in yarn production. Some of thevariables are listed below:(1)Type of fibre(s) and / or filament(s) used in an individual yarn.(2)Dimensional and physical characteristics of the fibre or filament used in ayarn e.g. fineness, cross-sectional shape, crimp, density, etc.(3)The mechanical properties of a fibre or filament e.g. tensile strength,tenacity, extensibility, elastic properties, etc.(4)The general properties of a fibre or filament e.g. frictional properties,moisture regain, thermal properties, dimensional stability, resistance to micro-organisms, static properties, electrical properties, colour, ageing etc.(5)Chemical properties of a fibre or filament e.g. resistance to acids, alkalis, drycleaning agents and other chemicals.(6)The method of yarn production e.g. carded system, combed system, woollensystem, worsted system, etc.(7)Method of final yarn formation e.g. ring, rotor, wrap, core, air jet & frictionspinning, etc.(8)Component of the yarn e.g. 100% natural fibres, 100% manmade fibres,blend of natural fibres with manmade fibres, blend of natural fibres withfilaments, etc.(9)The linear density i.e. the count of the yarn and the level of twist (twistmultiplier).(10)Cross-section of the yarn e.g. circular, elliptical, flat, textured, etc.(11)Ply of the yarn whether the yarn is single-plied or multi-plied.As far as natural fibres are concerned, they have typical properties dependingupon the group to which they belong. For example cotton, flax, jute, etc all arecellulosic fibres on the other hand wool, silk, mohair, etc all belong to proteinicfibres. There is nothing much can be done to alter the basic properties of thesefibres. These properties also vary from lot to lot within the same category. Onthe other hand in manmade fibres, most of the properties can be controlled to agreat extent and precision. They can both occur in filament and short stapleform of desired length.Consequently the yarn properties made of natural fibres are dependent on thebasic natural properties of the fibre. However in case of manmade yarnsproperties of the fibres can be modified to meet the requirements of the end useof the yarn.General Principles of Short Staple Spinning
14. All short staple yarn spinning systems make use of the following basic principles:(1) MixingThe term mixing is applied for combining or blending more than one mass offibres into a single homogenous mass. Since all the natural fibres vary from oneanother from region to region, field to field and even from bale to bale, it isnecessary to mix them well so that the final end product i.e. the yarn may behomogenous and of consistent quality.(2) BlendingUsually blending refers to the mixing and combining two or more than two fibresof different origins. For example cotton fibres with polyester. The purpose ofblending is to achieve desired properties of both the components of the fibres ina yarn which otherwise is unobtainable from a single component. For examplestrength, crease resistance, colour, price, moisture absorption, dryingproperties, etc.Just as mixing, blending should also be done thoroughly so that a homogenousyarn may be produced out of the component fibres.(3) OpeningThe raw fibres for easy transportation are highly compressed into bundles calledas bales. Before effective spinning can be carried out, this compressed form offibres must be separated from one another. Opening refers to mechanicalseparation of fibres from one another. The opening is carried out gradually insteps. In the first step the bale of fibre is broken down into small tufts then lateron at various stages of spinning these tufts are further broken down intoindividual fibres.(4) CleaningAll the natural short staple fibres have some amount of natural impurities in it.These impurities have to be removed before fibres are converted into a yarn. Onthe other hand the short staple manmade fibres just require opening but nocleaning.The amount and type of cleaning required for a particular lot of fibres dependsupon size and amount of impurities present in it. Greater the trash content infibres greater number of cleaning points are used during various stages of thespinning process. Typically cotton bale contains about 5 to 10% impurities andabout 3.5 to 7 % cleaning is obtained during initial opening and cleaning.Cleaning is generally associated with opening. As the fibre opening takes place,the impurities also get separated and removed. Greater the degree of opening,greater cleaning may be carried out.(5) Fibre Separation
15. The fibre separation is the further opening of the small tufts that have beeninitially opened up into an individual fibre form. This happens at the cardingmachine. By fibre separation a further up to 1% waste can be removed.(6) Fibre RegularisingFibre regularising means the reduction in the variation of the mass per unitlength of the fibre material. Regularising is very important to produce a regularand a more consistent quality of a yarn. Fibre regularity takes place at thedrawing frame.(7) Fibre AlignmentAlong with the improvement of the fibre regularity, the alignment of the fibresalso improves at the draw frame. Fibre alignment means the straightening of thefibres and making them parallel to the axis of the sliver.(8) DraftingDrafting is drawing out or attenuation of the fibre material into a desiredfineness or count of a yarn. In ring spinning system drafting is done in twostages one at the roving frame and other at the ring frame.(9) TwistingTwist plays a vital role in the final formation of the yarn. The purpose of givingtwist is to bind the fibres together as a yarn and to give strength to the yarn.The major twisting takes place at the ring spinning frame or at the final stage ofspinning.Cotton Impurities
16. Any foreign material other than fibres is classified as impurities. Not only thequality and the price of fibres depend upon the amount of impurities present inthe fibres, also the subsequent processes depend on it. Greater the impuritiesare more efforts have to put in to remove it. The removal of the impurities alsoresults in the loss of useful fibres. Impurities are also found in the manmadefibres however the level is significantly low as compared to impurities in naturalfibres.The impurities in cotton fibres can be classified into:(1) SeedSeed impurity is the largest type of impurity present in raw cotton and itincludes un-ginned seeds with fibres attached to it, ginned seeds and parts ofseeds.(2) ChaffThe chaff is the vegetable fragments consisting of leaf particles, bract, shale andstalk of the cotton plant. Bract is a small type of a leaf that grows beneath thecotton boll and shale is the silvery interior lining of the cotton boll.(3) DirtThe dirt impurity includes soil and sand particles that may be added from thecotton fields due to mishandling of the fibres and also the cotton fibres pick updust and sand if they are transported by open trucks.(4) Micro-dustThe micro-dust includes very fine particles of chaff, dirt, small fibre fragmentsand spores of mildew. These particles are extremely small and are often afraction of the fibre diameter. They generally gets embedded around the naturalwax of the cotton fibre.(5) Abnormal ImpuritiesThe abnormal impurities are very rare however when found in the cotton fibres,they can cause serious problems. These impurities include pieces of stones,pieces of iron, cloth fragments, foreign fibres such as jute, polypropylene, etc(that may be included due to the bagging of cotton fibres made up of thesefibres), grease and oil (from machine harvesting or ginning), tar and coal (fromthe air while the cotton fibres are transported openly), small pieces of wood, etc.The term trash is applied to all of these impurities present in the raw cotton. Thetotal trash content of cotton fibres ranges from 1% to 10% of the total weight ofthe cotton fibres. The amount of trash content directly determines the amount ofcleaning required.Removal of Impurities
17. The removal of impurities is associated with the opening of the fibres and iscarried out in stages during the spinning process. Initially the impurities areremoved in the blow room with the very basic opening of the larger tufts offibres into smaller tufts. Then further at the carding machine due to fibreseparation, more impurities are removed. The blow room mostly removes theseed and chaff while the carding removes the dirt and microdust. Greater theimpurities present in fibres more opening and cleaning is required. However withmore severe opening and cleaning, expensive fibres can be damaged or they canbe lost during the process.Methods of Opening & CleaningThe mechanical techniques or methods used for the opening and cleaning of thecotton fibres are:(1)Spiked SurfacesThis action consists of plucking and gripping the mass of cotton fibres betweentwo sets of spiked surfaces moving in opposite directions. This action opens thefibres and does some cleaning as well. Tearing Up Plucking Up Plucking Out(2) BeatersThe term beater in spinning is generally referred to a revolving drum havingblades, spikes or pins mounted on it surface. The fibres are fed and subjected tothe surface of the beater with the help of air currents or by using pair of rollers.When the surface of the beater strikes the fibre mass, it plucks or tears thefibres and transports the opened fibre to next stage. During this opening, thetrash being heavier falls down and is collected below the machine. Plucking Out Tearing Out Beating Out
18. Bladed Drum Roller with Toothed Discs Bladed Drum(3) Air Currents (Pneumatic Action)Lighter impurities like dust and micro-dust can not be effectively removed fromthe fibres by using either the spiked surfaces or beaters. These impurities can beremoved by passing the fibres over the perforated grids where the air currentscan draw off the dust in the fibres.All the above and majority of the operating devices in the blow room machineryare opening devices when they are used alone. However these very sameopening devices can also work as cleaning devices if they are worked incooperation with cleaning apparatus such as grids and special machine covers.The following elements can be used in grids: (i) Slotted Sheets (ii) Perforated Sheets (iii) Triangular Section Bars (iv) Angle Bars (v) BladesThese elements can either be used alone or in combination with each other. Forexample, the perforated and slotted sheets were widely used and placed underthe cards but now there use is diminishing. Same is the case with the blade gridsthat were used in combination with triangular bars grids.
19. Perforated Sheet Slotted Sheet Triangular Bars Angle Bars Knife BladesThe angle bars are very robust but they tend to create fibre blockages. So Todayin the modern cleaning techniques, either the triangular grid bars or knife bladesare used alone for the most efficient waste removal.The impurities and the fibres fall through the gap of the grids and are collectedin a special waste chamber of the machine which is placed under the grid. In oldmachinery this waste has to be manually removed periodically however in thelatest opening and cleaning systems pneumatic waste removal systems areused.Grid AdjustmentsThe grids can be in one, two or three parts so it can be adjusted as a unit or inindividual sections. Three basic adjustments are possible. (i) Distance of the complete grid to the beater. (ii) The distance or the gap between the adjacent grid bars. Closed Gap Setting Open Gap Setting (iii) Angle relative to beater blade Oblique Angle Aggressive AngleIt is seldom possible to make all these three adjustments, generally machinesare so designed that only two adjustments are possible.
20. Cleaning EfficiencyAll openers & cleaners along with foreign matter also remove a certain amountof short fibres (also called as lint). The composite of trash, dust, fibre fragmentsand fibres removed is called as waste. The amount of waste removed at eachstage of cotton cleaning stage should be known for evaluation and can be foundout as: Waste Removed (Kg) % age Waste Removal = x 100 Total Fibres Processed (Kg)The effectiveness of a machine or series of machines in a blow room to removethe trash in the fibres is expressed as its cleaning efficiency and is given by: % trash in raw fibres - % trash in processed fibres%Cleaning Efficiency = x 100 % trash in raw fibresFactors Influencing Opening & CleaningThe degree of opening, the degree of cleaning and the fibre loss are primarilydependent on the following factors:(1) The type of opening devices used.(2) The speed of the opening devices.(3) Type of feed(4) Degree of penetration.(5) Spacing of feed from the opening devices.(6) Type of grid used.(7) Area of grid surface.(8) Grid Settings.(9) Airflow through the grid.(10) Condition of pre-opening.(11) Position of the machine in the machine sequence.THE BLOW ROOM
21. The blow room is the first stage or the first process in the short staple spinning.The name ‘Blow Room’ is given to this stage because of the air currents that arecommonly used during the processing of fibres. the blow room the fibre mass isprogressively opened, cleaned and mixed. This is done by using a large numberof machines. In each of these machines used in blow room if the actions are toosevere of sudden then fibre damage will occur.Functions of Blow Room(1)Fibre Opening: The tightly packed fibre bales received from the ginning millshave to be opened by converting the larger fibre tufts into smaller ones andultimately converting the smaller tufts into individual fibre form.(2)Cleaning: All the natural fibres including cotton have considerable amount ofimpurities in them which have to be removed to produce a clean yarn.(3)Mixing/Blending: The properties of the cotton fibres differ from each otherfrom bale to bale and from fibre to fibre so in order to obtain a homogenous andconsistent quality yarn, they need to be thoroughly mixed together. Sometimesin order to have a desired quality at the right price high quality cotton fibres aremixed with low quality fibres.(4)Preparation of feed for the next stage: The end product of the blow roomshould be compatible with the next stage of spinning i.e. carding. The feed tothe carding can be either given in the form of lap or in direct chute form.Blow Room MachineryIn the blow room all the above functions have to be fulfilled for this purposevarious different types of machines are used. Based on the functionality of thesemachines they are classified into five types:(1) Bale Opening Machines(2) Mixing Machines(3) Cleaning Machines(4) Dust Removing Machines(5) Recycling MachinesFor these machines to perform optimally, they must be located at specificpositions in the blow room line. The modern cotton blow room line can bedivided into six distinguished zones.(1) Bale Opening Zone(2) Coarse Opening & Cleaning Zone(3) Mixing/Blending Zone(4) Fine Opening & Cleaning Zone(5) Intense Opening & Cleaning Zone(6) Card Feed Preparation ZoneIn case the cotton has less impurities then the Zone 5 (intense opening &cleaning) may not be necessary. Furthermore the Zone 4 (fine cleaning) or the
22. Zone 5 (intense opening & cleaning) and the Zone 6 (card feeding) can form asingle unit.The additional operation of dust removal is not associated with any single zone;in fact dust removal is carried out at a greater or lesser extent at every machineof the blow room.Bale ConditioningThe cotton fibres from the ginning factories are received by the spinningdepartment in form of highly compressed bales that are wrapped by metal orplastic straps. As the bales are received these straps are cut off and the balesare allowed to condition for 24 hours in controlled temperature and between60% to 80% relative humidity. For this purpose all the spinning mills allocatefloor space for conditioning purpose.The conditioning allows the fibres to relax and maintain a temperature andmoisture equilibrium with atmosphere and reduces the chance of fibre damageand inconsistency in quality.Bale Lay DownAfter the bales are conditioned properly they are taken to the blow room andplaced in groups of special sequence for the first processing stage. This group ofbales is called as bale lay down. The main aim of a proper bale lay-down is tohave fibres with similar properties and spinning attributes from lay-down to lay-down so that spinning machines can be adjusted optimally and yarn ofconsistent quality may be produced over a longer period of time.Zone-1 (Bale Opening Machines)After proper bale lay-down the initial bale feeding is done either by using aparallel set of machines called as hopper feeders or by a single machine calledas a top feeder. The hopper feeders have stock supply compartments which areeither filled manually or by automatic machines. A cross-sectional diagram of atypical hopper feeder is shown below: (1)Feed Table (2)Internal Feed Lattice (3)Light Barriers (4)Baffle Plate (5)Brush Rolls (6)Spiked Lattice (7)Cleaner Roller (8)Evener Roller (9)Stripper RollerThe more realistic shape of the hopper feeder can be seen in the followingfigure:
23. The hopper feeders although are still used in quite sophisticated form however they are considered to be conventional type of bale openers. They remain stationary while the raw fibres from the bales can be fed manually or by automatic machines. Nowadays the most popular and modern machine for feeding raw fibres from the bale is the top feeder. In the following Figure, the Rieter Unifloc Top Feeder is shown:(1)Electrical Feed Cabinet(2)Channel For Electric Cable(3)Covering Belt(4)Take-off Unit(5)Swivel Tower(6)Control Panel(7)Evacuation Duct(8)Drive Rails(9)Chassis The top feeders are travelling machines that move over and past the bale layout and extract fibres from top to bottom. They have great advantage that more than one bale can be processed simultaneously to give a better long term blend. These machines are fitted with computerized control panels and they extract material from all the bales evenly. The production rates of such modern bale openers ranges from 750 kg/hour to 1000 kg/hour The hopper feeders and the top feeders should perform the following functions:
24. (i) Extract material evenly form bales.(ii) Open the material gently.(iii) Open up to smallest tufts.(iv) Form tufts of equal sizes.(v) Process as many bales as possible in a single charge.(vi) Easily programmable.(vii) Blend fibres at the start of the process.All the bale opening machines not only feed the raw fibres but also do the tuftopening. This opening actually starts from the point when these feeders startgripping the fibres for an initial feed as shown below:Zone-2 (Coarse Cleaning Machines)
25. The coarse cleaning machines directly gets it feed from the hopper feeders orfrom top feeders. The striking and beating elements in this zone are widelyspaced and hence the opening of the fibres is also very minimal. The mainpurpose of these machines is to open up the mass of fibres into large tufts whichare then converted into smaller tufts by using more intense opening andcleaning machines in the next zones. The machines in these zones aresometimes not even fitted with cleaning devices or even if these cleaningdevices are present, they can only remove fraction of the impurities.Different machine manufacturers have developed various types of coarsecleaning machines. The most commonly used ones are:(i) The Step CleanerThe step cleaner is a very standard type of a coarse cleaning machine that isproduced by several manufacturers. Truetzschler Step CLeanerAs the material falls into this machine it is subjected to first beater which notonly does the initial opening but also transports the fibres upwards wheresometimes 4 or 6 beaters are placed closed to one another and inclined at anangle of 45°. The surface of these beater rollers are covered with blades or bars.The cleaning of the impurities takes place as the material continuously passesfrom one roller to the other with the help of grids placed beneath each of theroller. The speed of the beaters and the grids are both adjustable.(ii) Uni-Cleaner
26. The uni-cleaner or the mono-cylinder cleaner relies on the use of single beaterroller having its surface covered with spikes. The fibre material enters to themachine from one side due to a suction effect produced at the other side of themachine. To ensure that fibres may not pass the exit pipe untreated by thebeater, following arrangement is done:(a) The hood of the machine around the beater is designed in three portions in such a way that the fibre mass is forced to fall back into the region of the beater after being beaten by the beater. In this way the fibres are forced to circulate the beater many a times to give required opening and cleaning.(b) The exit opening of the machine is kept higher than the in-feed opening of the machine that also ensures that only the smallest tufts can pass straight through but the bigger tufts are always subjected to the beater action of the beater. Rieter Monocylinder Cleaner(iii) The Dual Roll Cleaner
27. The dual roller beater is some how similar in working as that of a mon-cylindercleaner. However in this case instead of only a single beater roller, two beaterrollers of about 61 cm diameters are used. Both of the rollers rotate in the samedirection and have their surfaces covered with spikes arranged in a spiral toimprove passage of the material. Hergeth Hollingsworth Dual Roller CleanerThe exit opening of the machine is kept higher than the in-feed opening of themachine to ensure that only the smallest tufts can pass straight through but thebigger tufts due to weight falls down and are always subjected to the beateraction of the beater.(iv) The Three Roll CleanerThe three roll cleaner is exactly the same in working as the dual roll cleaner. Theonly difference is that it has three rollers placed side by side instead of two. Crosrol Three Roll Cleaner
28. Zone-3 (Blending/Mixing Machines)(i) The Mixing BatteryThis is the most commonly used type of a mixing/blending machine that doesthe mixing at the start of the process. In the arrangement 2 to 6 bale openersare operated together independently. The opened fibre material form all the baleopeners are fed onto the common conveyer belt.This gives a very good mix and blend of fibres. In the latest mixing batterieseach of the bale opener is equipped with electronic weighing equipment that caneasily ensure correct blends of various components of fibres at a predeterminedratios e.g. example 60% Cotton, 40% Polyester.(ii) The Multiple MixerThis is again a very simple mixer that gives very good long term blend. Themachine is composed of several (6 – 8) chambers. The fibre material ispneumatically fed from the top. All the chambers are successively andsimultaneously filled and the material is removed from the bottom through asingle common duct. (1)Fan (2)Air Bypass (3)Exhaust Air Duct (4)Pressure Switch (5)Feed Duct (6)Closing Flap (7)Perforated Plate (8)Blending Chamber (9)Light Barrier (10)Delivery Rollers (11)Opening Rollers (12)Blending Channel (13)Suction Tunnel (14)Exhaust Air Outlet Truetzschler Multi-Mixer
29. (iii) The UnimixThe unimix is a combination of blending and cleaning machine and both of thesetwo operations are carried out within the single machine. Rieter Unimix(1)Feed Pipe (2) Filling Chambers (3) Conveyer Belt(4) Conveying Roller (5) Upright Lattice (6) Intermediate Chamber(7) Stripper Roller (8) Take-off Roller (9) Filling Trunk(10) Cleaner Roller (11) Waste Chamber (12) Fiber Delivery(13) Exhaust Piping (14) Exhaust Air OutletThe machine is divided into three sections: (a) Storage Section (b) Intermediate Chamber (c) Delivery SectionThe fibres are pneumatically fed into six individual chambers of the machine.The fibres coming out of each of the six chambers are taken on a common latticeor a conveyer belt that takes the material to an intermediate chamber with thehelp of an inclined or upright lattice. From here the material passes through adelivery section to the next machine with the help of a pneumatic suction. In thedelivery section a cleaning roller is used which does the coarse cleaning of thefibres as they are being delivered.
30. Zone-4 (Fine Opening & Cleaning Machines)The Zone 4 cleaning machines although utilizes the same principles of openingand cleaning as that of the Zone 2 cleaning machines but has some differences: (a) The Zone 4 machines are always fed using clamp feed that is to make sure that controlled amount of fibre size and fibre quantity is fed. (b) The spacing of the beater with the hood of the machine and with the grids is kept finer. (c) Finer and more number of striking elements (pins, blades, spikes, etc) are used. (d) The speed of the beaters is kept higher.The RN Cleaner of Truetzschler as shown below is one of the most efficient andwidely used fine opener and cleaner: (1) Condenser (2) Dust Cage (3) Fan (4) Finned Roller (5) Feeding Unit (6) Light Barrier (7) Feed Rollers (8) Step Cleaner (9) Cleaner Roller (10) Microdust Suction (11) Fresh Air Flaps (12) RN Cleaner (13) Inner Lattice (14) Pressure Roller (15) Feed Rollers (16) Porcupine Beater (17) Two-Part Grid (18) Air InletIn the above figure the feed to the RN cleaner is given directly from the stepcleaner (zone 2) onto a feed lattice. The pressure roller and the pair of feedroller help to give a steady and predetermined feed of the fibres to the beater.The surface of the beater is covered with metal blades and has double hardenedworking edges. Beneath the beater two grid bars are placed that covers half ofthe circumference of the beater. These grids are fully adjustable.
31. Another very fine example of fine opener and cleaner is a Rando Cleaner asshown below: Rando Cleaner By Carolina Machine Co.This opener and cleaner perform its working by using multiple rollers havingtheir surfaces covered with saw teeth. All of these rollers move in oppositedirection to one another and hence does the opening and cleaning by not onlythe beating action but also due to the opposing spikes principle.
32. Zone-5 (Intense Opening & Cleaning Machines)In majority of the cases the Zone 5 machines utilizes either the Kirschner beateror the carding roller (roller covered with saw teeth) as the main opening andcleaning device. However the way and the place where these opening rollers areused vary from manufacturer to manufacturer. A widely used intense opener andcleaner is the Rieter ERM cleaner as shown below: (1)Material Supply (2)Feed Head with Fan (3)Exhaust Air Piping (4)Material Delivery (5)Material Chute (6)Plain Drum (7)Dust Cage (8)Feed Rollers (9)Knife Grid (10)Beater (11)Suction Duct (12)Waste Chamber (13)Driving Motor (14)Waste Removal PipeHere again a fan is used that sucks the fibres processed from the previousmachine of the blow room line into the filling chute or filling chamber of thismachine. The mass of fibres is condensed with the help of drum roller and pairof feed rollers and is subjected to a drum beater whose surface is either coveredwith saw teeth or bladed discs. The beaters thoroughly opens the fibre materialand transports it to the next stage by suction, while the trash removed duringthe beating and opening action passes through the grids blades and is collectedin the waste chamber.Another type of an intense opener and cleaner is shown below: (1)Feed Lattice (2)Pressure Rollers (3)Feed Rollers (4.1) Pinned Roller (4.2) Needle Roller (4.4) Saw-Tooth Roller (4.5) Fine Saw-Tooth Roller (5) Knife With Suction (6) Carding Segment
33. Truetzscher CleanomatZone-6 (Card Feed Preparation Machine)Card Feed Preparation ZoneThe feed to the carding machine is possible in two ways i.e. pneumatic chutefeed with fibres in opened form and lap feed with fibres in form of a sheet orweb. However whatever the feed method is used, it is essential that the feedingmaterial to the card should be homogenous over a long term period. In thisregard the lap feed is generally preferred because: (1) The lap feed to the card is less problematic and it is much easy to control the homogeneity of the lap as compared to chute feed. (2) It can be easily operated with several blends.With these advantages the lap feed also has some serious disadvantages: (1) Greater manual effort is required to transport the lap roller. (2) Laps can be an additional source of faults. (3) When the lap roller becomes full it has to be replaced by a new empty one, it also requires extra effort. (4) Since laps are heavily compressed, it puts additional burden on the carding machine.Because of these serious limitations all the modern cards are fed with chute feedrather than lap feed. However if lap feed is to be prepared, it is done on amachine called as a scutcher as shown below:(a) Perforated Drum (b) Pocketed Roller (c) Fan(d) Photocell (e) Reserve Chute (f) Take-off Rollers(g) Opening Roller (k) Feed Chute (m) Kirschner Beater(n) Calender Rollers (o) Lap Tube (p) Winding RollerThe main objectives or functions of a scutcher machine are: (1) Opening (2) Cleaning (3) Regulating
34. (4) Lap FormationTypically a scutcher machine can be divided into the following regions: (1) Feeding Region (2) Opening & Cleaning Region (3) Lap Forming Region (4) Lap Doffing Region(1) Feeding RegionWith the help of air suction produced by a suction fan (c), the fibre material formthe previous machine enters the scutcher machine and is drawn against aperforated drum (a). The drum revolves rapidly and removes the air from thefibres and hence does some dust removal. A pocketed roller (b) strips off thefibres from the perforated drum and throws it to the reserve chute (e). Aphotocell (d) is used in to maintain the amount of fibre present in the reservechute. At the bottom of the reserve chute with the help of the two pairs of take-off rollers (f) and an opening roller (g), the fibre mass is thrown into a narrowfeed chute (k). During the transport of the fibres in the feed chute high airpressure condenses the fibre mass into a form of a strand or a web. A pressuremeasuring and control system ensures a steady air pressure and air flow so thateven strand of fibres may be obtained.(2) Opening & Cleaning RegionThe opening and cleaning region of the scutcher line is carried out by using aKirschner beater. The feed to the beater is given in a very controlled manner byusing a feed roller and set of pedal levers. 18 set of pedal levers form a feedplate. The levers press the fibres web with the feed roller with a uniformpressure that changes the thickness of the web. Any variation in the thickness ofthe fibres web will cause the lever to move up and down. This up and downmovement of the lever is translated to alter the speed of the feed rollers so thata constant thickness of the web may be obtained.The grid under the Kirschner beater is made up of number of triangular bars(most commonly 10) out which the first few can be adjusted independently whilethe others are adjusted n groups.(3) Lap Forming RegionThe lap formation takes place with the use of a perforated drum (a) thatremoves the air currents by sucking them into its perforations. As the perforateddrum rotates, a single layer of a compact lap is formed on the surface of thedrum.The layer of lap produced on the drum is removed with the help of specialstripping rollers and is then subjected to set of three calendering roller with onelarge calender roller placed on top of the other two calender rollers. Thecalendering rollers exert a constant equally distributed pressure up to 6000 kg.Because of this high pressure the lap is uniformly condensed and its thickness isreduced. The compressed lap is then wound on a lap tube (o) with the help oftwo winding rollers (p). The winding rollers also exert a pressure of about 1000
35. kg so that a condensed lap roll may be produced having a diameter up to 55 cmand it weighs up to 40 kg.The scutcher machines are also fitted with lap weighing devices that monitor theweight of the lap roll. Any variation in the weight of the lap from a preset valueis registered and based on the variation a signal is given to the servo motor thatcontrols the speed of the machine. If the weight of the lap roll increases thespeed of the machine is increased and vice versa.(4) Lap Doffing RegionWhen a lap of required diameter and weight is formed then that completed laproll must be replaced by a new empty one. This replacement of a full lap roll byan empty one is called as doffing. Doffing can either by carried out manually byworkers or in modern machines it is done by automatic doffing units.Dust Removal at Blow RoomDust and microdust are the finest particles of trash. Their removal takes place atvarious stages in the blow room. Two techniques are mostly used for theremoval of dust:(1) By separating the fibres and releasing dust into air, this dust is then removed by removing the dust contaminated air. The release of dust occurs whenever the fibres are rolled, beaten or opened up. In this type of arrangement its not only important to remove the dust contaminated air but also extremely important to maintain a dust free atmosphere in the blow room.(2) By separating the dust particles directly from the fibres through suction and scarping. This arrangement is better as compared to the first one as chances of dust to fly in the atmosphere are not present. Many different techniques are used to separate the dust from the fibres, most common ones are: (i) Use of perforated drums. (ii) Use of Stationary Perforated Surfaces. (iii) Circulating perforated belts. (iv) Stationary combsThe perforated drums and perforated surfaces are the most commonly usedtechniques for dust removal. For example, in the following diagram a Rieter dustextractor is shown that make use of stationary perforated surfaces.
36. The equipment includes a specially designed converging pneumatic duct havingperforations on its either side. This duct is enclosed in a chamber. As thematerial passes through the duct a strong suction fan draws off the fine dustparticles from the fibres.In the following figure Truetzschler dust extractor is shown that make use ofrotary perforated drum:Here the incoming material is drawn on a perforated drum with the help of airstream. This air stream is then removed by using a high vacuum exhaustthrough the drum perforation using a suction fan. By doing so, fine dust alsogets removed along with the air. The fibre material is stripped off the perforateddrum with the help of a paddle roller. The stripped fibre material is thentransported to next stage with the help of a suction provided at that end.Cleaning Efficiency of Blow Room
37. The effectiveness of a machine or series of machines in a blow room to removethe trash in the fibres is expressed as its cleaning efficiency and is given by: % trash in raw fibres - % trash in processed fibres%Cleaning Efficiency = x 100 % trash in raw fibresAnother very practical equation to find the cleaning efficiency is: % Waste Removed x % Trash in Waste %Cleaning Efficiency = x 100 %Trash in Raw FibresHow Much Waste To RemoveAll openers & cleaners along with foreign matter also remove a certain amountof short fibres (also called as lint). The composite of trash, dust, fibre fragmentsand fibres removed is called as waste. Depending upon the machine design andintensity of opening and cleaning used, the removed waste has 40% to 70% offibres by weight in it. So more fibres present in a waste makes the process morecostly. To estimate the amount of waste that must be removed in the blow roomin order to achieve a prescribed level of cleaning, following equation can beused: % Trash in Bales X % Trash to Remove % Waste Needed = x 100 % Trash in WasteThe amount of waste removed at each stage of cotton cleaning stage should beknown for evaluation and can be found out as: Waste Removed (Kg) % age Waste Removal = x 100 Total Fibres Processed (Kg)Openness MeasurementThe opening effectiveness of a machine or series of machines in a blow room linecan be found out by finding the openness index. The openness index can befound out by using a simple apparatus developed by the Textile Institute. Theapparatus include a 4000 mm Pyrex beaker with inner diameter of 152 mm anda glass disc of 200 grams in weight. The glass disc has holes on its surface sothat air can escape and its diameter is slightly less than the inner diameter ofthe beaker. The apparatus is shown below:
38. In order to find the openness index, the following procedure is followed:(1) A random sample from processing point is taken with a care that openness of the fibre is not disturbed.(2) The Pyrex beaker is uniformly filled with the fibre sample.(3) The 200 grams disc is placed on top of the fibre with a care that disc should not settle at a sharp angle.(4) The volume of the compressed sample is noted down.(5) The disc is removed and sample weight is found out(6) The openness index is then calculated as: Volume of Fibres (ml) Openness Index = x Specific Gravity of Fibre Weight of Fibres (gms) In case of blended fibres, the blended specific gravity is taken as: Blended Specific Gravity = (Specific Gravity of Component1 x %age in Blend) + (Specific Gravity of Component2 x %age in Blend)
39. (7) In order to have accurate results 8 to 10 readings are taken.The following table shows the change in openness index of fibres after beingprocessed by various machines and components in the blow room line. Machine Change in Openness Index Hopper Feeder 40 to 50 Top Feeder 80 to 85 Coarse Opener & Cleaner 5 to 10 Fine Opener & Cleaner 15 to 25 Intense Opener & Cleaner 20 to 30 Mixer & Blender 0 Transport Fan 0Blow Room AccessoriesIn addition to the main machinery of the blow room many useful accessories arealso used such as: (1) Heavy Particle Separator (HPS) (2) Magnetic Metal Traps. (3) Fire Eliminator (4) Waste DisposalThe heavy particle separator (HPS) removes heavy particle like metal, plastic,wood, etc. These units take advantage of greater inertia of heavier particles inorder to remove them. For example in the following figure a heavy particleseparator is shown:
40. Similarly magnetic traps are also but will naturally remove only metallicparticles. These magnetic traps can either be used individually or in combinationwith the heavy particle separator (HPS). One such example is shown below:If these heavy particles are not removed before processing of fibres then at highspeed beaters, they may generate spark resulting in fire. Since the fibres areflammable they can cause lot of damage to the machinery and raw fibre andsometimes can also become life threatening.So in order to have extra protection in the blow room machinery, it is sometimesalso equipped with fire eliminators. The fire eliminator on detecting a spark or aburning material immediately transports the fibre material to stand in open air.Simultaneously an alarm is given and the blow room line is switched off.
41. THE CARDING PROCESSThe carding is a one of the most important process of the short staple spinningsystem. Carding is an operation where the tufty condition of the fibres isconverted into an individual fibre form. The separation of fibres in individualform is one fundamental operation of carding while the other fundamentaloperation is the formation of the card sliver. The carding is a very importantprocess because unless the fibres are separated into individuals, they can not bespun into smooth and uniform yarns neither can they be blended properly withother fibres.Functions of Carding(1) Opening: As the blow room only opens the fibre mass from larger tufts to small ones, the main objective of the carding machine is to further open up the smallest tufts into an individual fibre form.(2) Cleaning: The removal of impurities is also an important objective carried out by the card. Since not all the impurities are removed by the blow room, it is essential at the carding to remove the remaining impurities. Modern carding machines can remove about 85 to 95% of the foreign matter present in the fed fibres. The overall degree of cleaning achieved by both blow room and carding room can be as high as 95 to 99%.(3) Mixing & Blending: As the fibres are processed in the carding machine, they are not only opened up to the extent of the individual fibre form but also are thoroughly mixed together. Sometimes blending of two or more different types of fibres can take place at the carding machine. The card can be a very good point of blending as with the carding action an intimate fibre to fibre blending is achieved.
42. (4) Disentanglement of Neps: Because of the repetitive beating and opening of the fibres, the number of neps increases from machine to machine in the blow room line. The carding machine due to its special action on the fibres opens the majority of the neps and hence their number is reduced considerably.(5) Removal of short fibres: The carding machine also removes a very small quantity of short fibres. The amount of short fibres removed at the carding process is not more than 1%.(6) Sliver Formation: The end product of the carding machine is produced in a form of a cylindrical mass of fibres called as silver. The sliver is the very first intermediate product of spinning that start to resemble somehow like a yarn.(7) Fibre Orientation: Although not majority of the fibres in the card sliver are parallel and aligned however with formation of the card sliver, the fibres for the very first time becomes slightly parallel and assumes some longitudinal orientation. So the carding process also helps to create partial longitudinal orientation of the fibres.Types of Carding MachinesDepending upon the staple length of the fibres to be processed, two types ofcarding machines are available:(1) Revolving Flat Card(2) Roller and Clearer CardRevolving flat card is meant for short staple fibres with staple length up to 2inches. The name ‘Revolving Flat’ card is given because these cards make use offlats that revolve on an endless path. The cotton fibres are carded using therevolving flat card.The roller and clearer card instead of having revolving flats have number of pairsof working and clearing rollers based on which its name is given. The roller andclearer card is mainly used for woollen fibres and is also sometimes called aswoollen card.Flat Revolving Card and its Components
43. Description of Parts(1) Conveying Duct (2) Feed Chute (3) Feed Roller(4) Card Feed (5) Taker-in (6) Knife Grid(7) Suction Duct (8) Cylinder (9) Front Carding Segment(10) Flats (11) Cleaning unit (12) Post Carding Segment(13) Cylinder Grid (14) Doffer (15) Stripping Device(16) Calender Rollers (17) Can (18) CoilerPrinciples of WorkingThe carding action refers to passing of fibre material in between two moving wiresurfaces. This typical action is repeatedly carried out in the carding machine toindividualize the fibres. At various stages of the carding machine the fibres areforced to pass through closely spaced surfaces covered with sharp metal teeth.The use of these sharp pointed surfaces give rise to two types of actions:(1) Point to point action or Carding Action(2) Point to back action or Stripping Action
44. Carding Action Stripping Action(1) Carding ActionThe carding action is used to separate and individualize fibres. This action takesplace between:(i) Feed roller and taker-in(ii) Cylinder and flatsRequirements of Carding Action(a) There should be two moving wiry surfaces between which fibres are subjected.(b) The action between these two wiry surfaces should be point to point.(c) There should be a difference in the surface speed of these two surfaces. Greater the speed difference more carding power is achieved Carding Power = Surface Speed of Cylinder / Surface Speed of FlatsTo achieve best carding power, the speed of the flats should be kept as low aspossible. The optimum running speed of flats is about 4 to 6 inches per minute.To vary the carding power the surface speed of the flats is altered dependingupon the opening and cleaning required at carding.(d) The distance between the two wiry surfaces should be constant. For cotton fibres a gauge of 8/1000 to 10/1000 of an inch is used.(2) Stripping ActionThe stripping action is used to transfer the material from one place to the other.As the material is transferred by this action, opening and cleaning also takesplace. Stripping action takes place between:(i) Taker-in and cylinder(ii) Cylinder and doffer(iii) Doffer and stripping rollerRequirements of Stripping Action
45. (a) There should be two moving wiry surfaces.(b) The action between these two wiry surfaces must be point to back.(c) There should be a difference in the surface speed of two surfaces. However the difference in the surface speeds should not be as high as that in carding action. The recommended difference ratio is 1:2 i.e. the surface to which the material is to be transferred should have twice the surface speed.(d) The distance between the two wiry surfaces should be constant. For cotton fibres a gauge of 3/1000 to 7/1000 of an inch is used.Material Feed To The CardThe fibre feed to the card coming from the blow room can either be in the formof a lap or in chute feed form. Although the lap may have some advantages butbecause of the serious limitations associated with the lap feed, it is no longerused in the modern short staple spinning, instead the chute feed is preferred.The final machine in the modern blow room line also acts as a card feeder.Depending upon the amount of trash present in the raw fibres and the degree ofopening and cleaning, the card feeder can either be a fine opener & cleaner oran intense opener and cleaner. Whatever the case may be, after the fibres areprocessed by the final machine, the fibres are transported with the help of astock transport fan to the ducts and chutes that lead to the carding machine. Atypical stock transport fan is shown below:Generally one fine or intense opener and cleaner with a transport fan can givefeed to line of 6 to 10 cards.Transport Duct SystemsTwo basic transport duct systems are used commercially:(1) Re-Circulation System(2) Dead End System(1) Re-Circulation System
46. As shown above, in this system a fine or intense opener (1) with the help of astock transport fan (2) supplies the opened fibres in the direction of arrows to acircular pneumatic duct. A number of carding machines are connected to thiscircular pneumatic duct with the help of vertical chutes. In this system an excessof fibre is supplied to the duct and the stock of fibres that do not fall in thevertical card chutes is returned back to the opener to be re-circulated.(2) Dead-End SystemA typical dead-end transport duct system is shown below:As shown above, the system makes use of two separate fine openers each witha separate stock transport fan. Both of these openers feed the chute distributionduct from opposite sides. Since there is no re-circulation of fibres, thedistribution duct can be blocked between any two particular cards thus allowingtwo groups of cards to process simultaneously two different fibre stocksindependently. Blockage of the duct is achieved by used a simple slide platehaving pressure sensitive sensors. These sensors control the speed of the feedroller of the opener.
47. The dead-end system is widely used in modern installments because of thefollowing reasons:(iii) Fewer neps are generated.(iv) Fibre breakage is less.(v) The dead-end system has greater flexibility.(vi) Machinery instalment is easier.(vii) Feeding is easy and reliable.Operation of Revolving CardThe operation of the card can be divided into three main areas:(1) Feeding(2) Carding(3) Doffing(1) Feeding Region
48. Functions of the Feeding Region(i) Feeding of fibres to the carding machine at a controlled and pre- determined rate according to the speed and productivity of the card.(ii) Thorough opening of the fibres.(iii) Removal of impurities (cleaning).(iv) Transferring the fibres from the taker-in to the main cylinder.The Chute Feed SystemThe output of the carding machine i.e. card sliver should be regular and freefrom faults so that the resultant yarn made out of it can also be regular andconsistent in quality. This is only possible if feed given to card is even anduniform. If the card uses lap feed then even feeding may not be a problem sincethe lap is already checked for its count accuracy at the scutcher. However thechute feed is more sensitive and inconsistent. To obtain even chute feeding, thefibres in the chute should be equally thick, evenly distributed over the wholewidth of the card and should have same density all over. In its simplest form thechute feed to the card is shown below:This simple arrangement is called as a single chute system. Here the fibres arefed from the top. The fibres fall down due to gravity. A pair of delivery roller atthe bottom discharge the fibre stock on to the card feed table. This is aconventional system used in old machinery and has poor consistency. A betterand modern version of chute feeding system is the double chute system asshown below:
49. (1) Distribution Duct (2) Dust Extraction (3) Air Outlet(4) Reserve Trunk (5) Fan (6) Feed Roller(7) Opening Roller (8) Control Unit (9) Pressure Adjustment(10) Speed Adjustment (11) Pressure Sensor (12) Feed Trunk(13) Air Outlet (14) Take-off Rollers (15) Card Feed Roller(16) SpeedometerThis is a more sophisticated designed feeding system that makes use of a fan tokeep consistent air pressure on the fibre stock. A sensor is used that registerpressure variation on the fibres. If the pressure on the fibre mass increases, thespeed of the feed roller is also increased and vice versa. This helps to keep aconstant pressure on the fibres and hence a consistent fibrous stock ismaintained in the lower compartment and a controlled feed is given to thecarding machine.Card Feeding DeviceThe fibre stock at a consistent rate is fed to the feed assembly of the card. In itssimplest form, feed assembly is shown below:
50. This feed assembly comprises of a stationary feed table with a feed plate (1). Afeed roller (2) with a diameter of 80 to 100 mm is used that presses the fibresagainst the feed plate. The surface of the feed roller is covered with saw toothwire. The special design of the feed plate forces the fibre mass towards thetaker-in and the carding begins.Taker-in and its OperationThe taker-in roller has a diameter of about 250 mm having its surface coveredwith saw tooth. The speed of taker-in roller ranges between 800 to 1500 rpm.Beneath the taker-in an enclosure of grid elements for cleaning purpose areused.Working at 1000 rpm the taker-in provides 600,000 beating points per secondwith a circumferential speed of about 50 km per hour and a draft of about 1000is given. This severe point to point or carding action of the taker-in doesmajority of the fibre opening and about 50% opening of the entire cardingmachine is achieved here.CleaningThe extensive opening of fibres at the taker-in allows the removal of impuritieswith the help of cleaning aids placed beneath the taker-in. The cleaning aid inthe conventional card includes 1-2 mote knives and a grid whose half of the
51. surface is perforated sheet and the other half is slotted sheet. The impurities areremoved as the fibre mass at high speed strikes the knives and the grid. Inmodern cards to achieve high speeds instead of using grids triangular cardingsegments are used.Transfer of Fibres to Main CylinderBetween the surfaces of the taker-in and the main cylinder the condition of pointto back action or stripping action arises. Due to the stripping action, the fibrematerial is transferred to the main cylinder. As the fibres are transferred to themain cylinder, longitudinal orientation of the fibres takes place here. Thisorientation depends upon the ratio of the surface speed taker-in to cylinder,ideally this ratio should be 1:2. i.e. a draft of slightly above 2 is given at thispoint.Use of Multiple Taker-in RollersThe standard carding machine has only one taker-in roller. At higher productionrates to achieve good opening without fibre damage some manufacturers havecome up with a technique of using two or sometimes three taker-in rollers. Forexample Truetszchler DK-803 card as shown below utilizes three taker-in rollers:Three taker-in rollers are used so that at very high speeds, the opening of fibresmay be done gradually. This is done by:(v) Rotating all three taker-in rollers in opposition directions to each other.(vi) Keeping the speed of the each succeeding taker-in roller higher than the previous one (each roller runs 25% faster than the last one).(vii) Using finer tooth covering on each of three succeeding taker-in rollers to ensure steady flow and opening of material at high speed.(2) Carding RegionFunctions of the Carding Region(1)Intensive opening of the fibres into individual fibre form.
52. (2)Removal of the remaining trash and impurities.(3)Removal of short fibresCarding ActionThe major carding action takes place in the area between the main cylinder ofthe card and revolving flats. As the material is stripped off the taker-in towardsthe main cylinder, the fibre mass is subjected to severe carding action due to asignificant difference in the surface speed of the cylinder and flats.The flats move at a speed of about 4 to 6 inches per minute whereas thecylinder having a diameter of about 50 inches rotates at a speed of 150 to 600rpm. The cylinder of this diameter and speed produces a surface speed which isabout 10,000 times more than that of the flats. To alter the carding power, onlythe speed of flats is changed while the speed of the main cylinder remains thesame. The direction of movement of flats in old cards is kept towards the front ofthe machine while in modern cards it is kept towards the back. The direction ofmotion of flats has no effect on the carding power of the machine.For proper carding action, the space distance between the flats and maincylinder is very important. It should not neither be very great where cardingaction is compromised nor very less where fibre breakage may take place. Forcotton fibres usually spacing of 10/1000” and for polyester 17/1000” is used.Removal of Trash & Short FibresDuring the carding action between the flats and the main cylinder the waste getsembedded into the interspacing between the adjacent wires of the flats. Thewaste includes mainly the short fibres, neps, trash particles and dust. It istherefore very essential to clean off the surface of the flats so that the cardingaction between the main cylinder and the flats may not be affected. In oldcarding machines manual cleaning was carried out by stopping the machine aftera specific period of time (4 to 6 hours). However in modern cards the wasteremoval off the flats is carried out continuously with the normal operation.Carding PowerThe degree of carding or carding power achieved on a carding machine can beexpressed as: Carding Power = Rotary Speed of Cylinder / Surface Speed of FlatsSince the carding power does not only depend upon this ratio, so instead thecarding power of a card machine is more effectively expressed in terms numberof beating points presented per fibre. This can easily be found out by averagingtotal number of fibres being fed in specific time divided by the total beatingpoints presented in that same time. Carding Power = Beating Points per unit time / Fibres Fed in unit timeFor example in modern cards at the taker-in region there are about 0.3 beatingpoints per fibre in other words approximately every three fibres will have onebeating point. At the main carding region (between cylinder and flats) there are
53. about 10-15 beating points available for each fibre. So by comparing the numberof points available per fibre, true carding power is determined.The production rate of the modern carding machine has increased considerably.This means that more number of fibres will pass through the machine in anygiven time. In order to keep the same carding power, the number of beatingpoints must also increase proportionately. This is possible by:(i) Having more points per unit area (finer clothing) on the carding surface.(ii) Increasing the speed of the carding rollers(iii) Using additional carding segments.The clothing of the carding elements can not be changed to a great extentbecause a suitable distance must be given in between the two adjacent wires orpoints. For coarse fibres coarse clothing and for fine fibres fine clothing is used.Similarly speeds of the carding rollers can not be increased infinitely. Forexample the production of the card has increased from 25 kg/hour to about 75kg/hour. In order to achieve same carding power, old 300 rpm speed of thecylinder must be raised to 900 rpm. However this is not possible from bothdesign and technological aspects and there would be lot of fibre damage at thisspeed.So the only approach that is applicable for increasing the carding power is theuse of additional carding surfaces or carding positions. Two possibilities arepresent in this regard:(i) Increase in number of rollers used in carding machine.(ii) Use of additional carding segments.Use of Additional Carding SegmentsAdditional carding segments can be used in two positions in the cardingmachine:(1) Under the taker-in roller.(2) Between the taker-in and flats (pre-carding segment).(3) Between the flats and doffer (post-carding segment). Pre-Carding Segment Post-Carding Segment• The carding segment used under the taker-in region is to facilitate better removal of impurities.
54. • The pre-carding segment helps in an efficient transfer of the fibres from the taker-in to the main cylinder. It also ensures that fibres are transferred evenly and no lumps of fibres are allowed to pass to the main cylinder.• The post-carding segment is mostly used in conjunction with the mote knife. The short fibres, impurities and the dust passes through the small gap provided between the machine cover and the mote knife and are sucked off using a suction fan. This helps in removing further impurities during the operation in the card.(3) Doffing RegionFunctions of the Doffing Region(1) Transferring of fibres from the main cylinder on to the doffer.(2) Stripping the fibre web from the doffer.(3) Gathering the fibre web into a twistless strand (sliver).(4) Condensing or calendering the sliver.(5) Depositing the sliver into the sliver can.The Doffing OperationThe cylinder is followed by a roller called as doffer. The main purpose of thedoffer is to take the individual fibres coming from the cylinder and to condensethem to a web form. The diameter of the doffer is 24 to 27” and it rotates at aspeed of 20 to 60 rpm. The surface speed of the cylinder is about 20 to 25 timesmore than the surface of the doffer. This helps to create a thick layer of fibres onthe surface of the doffer. The action between the cylinder and doffer surfaces isshown below:Owing to a very low surface speed of the doffer, the rate of transfer of the fibresis only about 0.2 to 0.3 i.e. on average a fibre rotates 3 to 5 times around thecylinder before it is transferred to the doffer. In order to improve the transferrate, the spacing between the cylinder and doffer clothing is reduced to only3/1000” as compared to a standard stripping gauge of 7/1000”.The Detaching Apparatus
55. In old conventional card the detaching of the web from the doffer is done byusing an oscillating comb or doffer comb that moves up and down at a rate of2500 strokes per minute. However in the modern high performance cards, theweb of fibres from the doffer is detached by using a special detaching orstripping roller as shown in the figure above because the reciprocating motion ofthe doffer can not be used at higher speeds.The detached web is then passed between a pair of calendar rollers or crushrollers placed on one another. The surface of these rollers is smooth and apressure is applied in between these rollers. These rollers provide an additionalpoint of cleaning because any foreign matter present in the fibres can besquashed and dropped off at this stage. The crushed fibre web is finallysubjected to transverse belt sliver condenser. The opposite motions of thesetransverse belts convert the fibre web into a condensed strand of fibrescommonly known as sliver. Another way of converting the fibre web into a sliveris by using a specially designed trumpet guide as shown below:The special funnel shape of the trumpet guide forces the web stripped off thedetaching roller to be condensed into a sliver form.Depositing Sliver into Cans
56. The sliver produced by the card must be properly stored in packages called ascans. Normally can used for sliver storage are 48 inches with a diameter of 30,36 or 40 inches. The sliver coming from the transverse belt is passed through aspecial spiral motion of the coiler calendar rollers which helps to deposit thesliver in a spiral form. Cross-sectional View of an empty Sliver CanDuo or Tandem CardingAs the name implies the duo or tandem cards consist of two individual cardsjoined together as a single unit as shown below:
57. The doffer of the first card gives feed to the taker-in of the second card. Thedual carding action on the fibres has a positive effect on the quality and blendingof the fibres. Research has shown that tandem cards result in lower nep count,improved yarn appearance and also reduces yarn breakage during spinning.However the main disadvantages of the tandem carding are its very high initialcost, high power consumption and higher maintenance cost. Also since highperformance cards can give almost the same quality of carding as that oftandem carding, the higher cost of tandem carding is not justified for itscommon use. Due to this reason tandem carding has not become very popular.DraftThe degree of reduction in the linear density of the fibre material is called as thedraft. Draft can be expressed in two forms:(1) Actual or Technical Draft Actual Draft = Linear Density of Input / Linear Density of output(2) Mechanical Draft Mechanical Draft = Linear Speed of Output / Linear Speed of InputIf the percentage waste removal during the carding machine is (W) then theactual and mechanical draft are related to each other as: Mechanical Draft = Actual Draft (1 – W/100)
58. THE COMBING PROCESSCombing is an optional process in the processing of short staple fibres necessaryfor the preparation of high quality combed yarn. The process of combing iscarried out after carding and the combed sliver after passing through the drawframe follows the regular path of yarn formation.The carded sliver still has some trash particles, neps and short fibres in it. Inaddition to it, the individual fibres in the card sliver are not well alignedlongitudinally and majority of them have hooked surfaces. The basic purpose ofcombing is to remove short fibres and remaining impurities and to make thefibres well aligned and straight so that only long high quality long fibres are usedfor yarn making a yarn. The carding process brings out following positiveinfluence on the yarn character:(i) More uniform yarns and stronger yarns can be made as compared to carded yarns.(ii) Owing to greater cleanliness and alignment of the fibres, the combed yarns are much smoother and have better lustre as compared to carded yarns.(iii) Combed yarns are less hairy and compact as compared to carded yarns.(iv) Combed yarns can be spun into much finer counts as compared to the carded yarns. Counts finer than 40 Nc are usually spun with combing where uniformity and quality is required. However to make stronger yarns, even coarse yarns are spun by combing.(v) The combed yarn requires less twist as compared to carded yarns. So high quality knitted fabrics are also made from combed cotton to have better appearance and handle.The combing process therefore results in an improvement in the quality of theyarn and also enables the spinner to spin finer yarn counts. However the abovementioned quality improvements in the yarn are obtained at a cost of additionalmachinery, additional process, extra labour and extra floor space. This increasesthe cost of yarn production considerably.Functions of Combing(1) To separate the long fibres from the short ones. The longer fibres are processed into a combed sliver whereas the shorter fibres are removed as a waste. Depending upon the quality of the yarn required predetermined quantity of short fibres are removed during the combing process.(2) To eliminate the remaining impurities and trash left by the carding process. The waste combination of trash, short fibres and neps is collectively also called a noil. The amount of noil removed during combing ranges from 5% to 25% depending upon the quality of the yarn.(3) Elimination of majority of the neps in the fibre material(4) To straighten and align the separated long fibres.
59. (5) To create a combed sliver with maximum possible evenness. Degree of CombingThe quality of the combed yarn and degree of yarn fineness achievable dependsupon the type and quality of the raw material and degree of combing carried outduring the combing process. Based upon the degree of combing, followingdifferent combing processes can be employed in the production of a combedyarn:(1) Scratch Combing is carried out to produce lower quality of coarser combed yarns. In scratch combing only as little as 5% noil is removed. This slightly improves the quality of the yarn as compared to carded yarns. Scratched combed yarns are produced by using medium quality and medium lengths of fibres.(2) Half Combing removes noil in the range of 7 to 10%. Such degree of combing is again used for medium lengths of fibres.(3) Normal Combing is carried out in majority of the cases where fine quality of long fibres is combed with noil removal in the range of 10% to 15%.(4) Super Combing or Fine Combing is used for making best possible fine yarns. Here up to 25% noil is removed by using best quality Egyptian cotton.(5) Double Combing was once used with the finest Egyptian cotton to produce extremely fine counts of yarns. In this double stage of combing, noil up to 25% is removed. However this method is rarely used nowadays.Comber Lap PreparationSince the main function of combing is to remove short fibres, if the carded sliversare directly fed to the combing machine, the waste extraction would be very highand also lot of fibre breakage will take place. This is due to the fact that fibreorientation in the card sliver is very poor and also the card sliver has majority ofhooked surfaces. So it is desirable for the card sliver to be prepared into such aform which is suitable for the combing operation. For this reason a suitable lapwith straight and parallel fibres is formed which is presented as a feedingmaterial to the comber.The majority fibres in the card sliver have trailing hooks (about 50%). It hasbeen established with experience and experiments that better combing resultsare obtained when majority of fibres presented to the comber has leading ratherthan trailing hooks. This is because the leading hooked fibres can be straightenedout better and they pass into the combed sliver whereas the trailing hookedfibres have less chances of straightening and more chances of being removed asa noil. In order to straighten and align the fibres and also to convert the trailinghooks into leading position, even number of machines must be used in thepreparation of a comber lap and most commonly two machine processes areused. Straightening and orientation of fibres is achieved by using roller draftingmethod in both of the preparatory operations. The total draft of both themachines ranges from 8 to 12. Since the drafting tend to cause imperfectionsand unevenness in the material, operation of doubling is also carried out. The
60. doubling not only helps to improve the evenness of the material but also isnecessary to form a sheet of material which is converted into a lap.Methods of Comber Lap PreparationCommercially two systems of preparing the comber lap are used:(1) Lap Doubling System(2) Sliver Doubling System(1) Lap Doubling SystemIn the lap doubling comber preparation system the carded sliver is passedthrough a sliver lap machine followed by a ribbon lap machine.The Sliver Lap Machine (1) Creel or Feed Table (2) Drafting Arrangement (3) Web Gathering (4) Lap Formation (5) Automatic Lap TransportThe sliver lap machine is divided into the following regions:(1) Creel Region(2) Drafting Region(3) Winding Region(1) Creel RegionThe creel of the machine consists of two feed arrangements; each usually holds12 card sliver cans. All together it gives a doubling of 24. All card slivers afterpassing through series of guide rollers enter the drafting arrangement.(2) Drafting Arrangement
61. The sliver lap machine commonly uses a 4 over 4 roller drafting system with toproller pneumatically weighted. The pneumatic pressure can be adjusted up to1600 Netwons. A total draft of 1.3 to 3 is given at this arrangement.(3) Winding RegionThe sheet or web of fibres after being drafted out is passed over a guide plate ordeflecting plate which changes its direction towards four calender rollers. Thehigh compression (up to 16000 Newtons) created by the calneder rollerstransforms the fibre web into a lap. The lap then passes through two windingrollers that press against the lap tube with a pressure of 10000 Newtons andassists in winding of the lap on to the lap tube. The lap tube is placed on lapweighing devices which on the modern machines automatically removes the laproll when its required weight has been reached and is ejected on an automatictransport system that will take the lap roll directly to the next machine i.e.ribbon lap machine.The Ribbon Lap MachineThe basic concept of ribbon lap machine is same as that of the of the sliver lapmachine as shown below: Lap Roll Drafting Arrangement Deflecting Unrolling Plate Table Lap RollHere instead of a feed table a lap unrolling table is provided for 6 lap rolls. Thesheet unrolled from the lap passes through a standard 4 over 4 roller draftingsystem where a draft of 3 to 6 can be given. The drafted material after passingthrough calender rollers is wound by the winding assembly on a lap tube. Theribbon lap machines have an advantage that it gives a doubling of 6 in web formand thus high degree of evenness in transverse direction is achieved.The lap doubling system is considered to be old conventional system ofpreparing comber lap. But with the introduction of high performance modernmachinery the trend is tilting towards using a sliver doubling system rather thanlap doubling.
62. (2) Sliver Doubling SystemIn the sliver doubling process the carded sliver is given first passage through anormal draw frame and then series of drawn slivers are given second passagethrough a sliver doubling machine.Sliver Doubling MachineThe working principle of a modern sliver doubling machine also known as thesuper lap machine is shown below:The super lap machine has three feeding heads in the creel portion with eachhead holding 16 to 20 draw sliver cans. All the slivers coming from each feedinghead is passed through a vertically held 2 over 3 roller drafting system. The lapsheet formed by the combination of these drafted slivers are passed through apair of calender rollers and is ultimately wound on the lap tube with the help oftwo working winding rollers.THE COMBING MACHINEMany different types of combers are used for different fibre materials, comberscan be classified into following types:(1) Rectilinear Combers (used for cotton)(2) Circular Combers (used for worsted)(3) Rotary Combers (used for spun silk)(4) Hackling Machines (used for bast fibres)The rectilinear or cotton combers operate intermittently because the short lengthof the fibres does not allow continuous method of combing. One end of cottonfibre bundle is combed with cylinder comb or half lap having half of itscircumference covered with teeth while the other end is combed with single row
63. of needles called as the top comb. After both ends of the cotton fringe has beencombed separately, the separated fringes are reunited by a piecing unit. Thestandard parts of the comber are shown in the figure below:The combing of the cotton fibres is carried out in an intermittent cycle ofoperation called as the combing cycle. In one combing cycle, the short fibres areremoved and the long fibres are passed forward into a sliver. One combing cyclecan be divided into many phases(1) FeedingThe combing cycle begins with the feed of the lap. The lap sheet is fed to thecomber between the feed roller and smooth cushion plate also called as thebottom nipper. The top nipper or the nipper knife moves down to fix on thebottom nipper (cushion plate). Hence the lap sheet is gripped between the topand the bottom nippers. Lap unrolls for feeding Top nipper moves down(2) Cylinder or Half Lap CombingAs the lap is held by both the nippers, the half lap or the cylinder comb rotatesand the protruding fringe of the fibres is combed with the help of needlesmounted on the cylinder comb. Any fibres not held by the needles will be treatedas short fibres and will be removed as a waste during the rotation of the circular
64. comb. The waste (noil) is removed from the surface of the needle with the helpof a revolving brush mounted just below the cylinder. The waste removed is thencollected by suction at the back of the comber. Half Lap Combing or Cylinder Combing(3) PiecingAs the half lap or circular comb has finished combing and has cleared the fibrefringe, the detaching roller remains stationary and does not rotate however onlythe back top detaching roller rocks backward. At the same time the top nipper israised while the cushion plate or bottom nipper rocks forward. Also the feedroller rotates by a small and amount feeds a predetermined length of lap. Thisincreases the length of the lap fringe and as the bottom nipper moves forward,the leading edge of the lap fringe is entered into the nip of the detaching rollersand initiates piecing. During piecing the top comb also starts descending. Retracting of Top Nipper Detaching roller rocks backward(4) Top CombingJust as the piecing has started, a top comb with one row of needles is descendedinto the fibre fringe from the above. As the combed web of fibres is pieced orconnected to the surface of the detaching rollers, the detaching rollers now startrotating forward and the combed web of fibres is pulled through the top comb. Asthe fibres web is pulled through the top comb, short fibres, neps andentanglements not removed by the circular comb is removed here by the topcomb. As the bottom nipper reaches its maximum forward position, thedetaching is completed because the detaching rollers continue to move forwardwhile the bottom nipper begins to rock backwards. As detaching finishes the topcomb is withdrawn upwards
65. Top combing & Detaching Retracting of Top CombThe feed roller again rotates and advances a new short section of the lap to becombed by the bottom circular comb and the same combing cycle continues. New FeedingOn a modern comber the cycle of combing takes place 3 to 5 times in a second.(5) Sliver Condensing & DraftingThe combed web taken by the detaching rollers is delivered to the web panhaving a trumpet guide on its one side as shown below:The combed web is pulled through the trumpet guide with the help of a pair ofcalender rollers that converts the web into a combed sliver. The combed sliverscoming from all the heads of the comber are laid side by side and are passedthrough a draw box where a draft of 5 to 12 is given. Most commonly a 3 over 5
66. roller drafting is used where the rollers are inclined at an angle of 60°. Thedrafted slivers are coiled into sliver cans. On modern combing machines, thesliver cans are automatically doffed on completion.THE DRAWING PROCESSThe carding process is one of the most important process in short staplespinning as it separates fibres into individual form and also removes theremaining portion of impurities left by the blow room. Despite of manyadvantages of the carding process it has a big draw back of producing variationand misalignment of the fibres with in the card sliver. The alignment and theslight parallelization achieved at the carding region between the main cylinderand flat largely disappears again because of the doffing action at the doffer.During the transfer of the fibres from the cylinder to the doffer hooked surfacesin the fibres arise. About 50% of the fibres in the card sliver has trailing hooks,15% fibres have leading hooks and 15% of the fibres have double hooks andonly a small portion (20%) of the fibres remain straight.In order to produce a strong and uniform yarn it is necessary to straighten andalign the fibres and to improve the evenness of the sliver. All of these objectivesare achieved by the drawing process carried out by a machine called as the drawframe. At the draw frame a number of card slivers are drawn or stretchedbetween several pairs of rollers. As the fibres are attenuated or drafted, thefibres are straightened and aligned to the axis of the sliver in the direction inwhich they are drawn.Functions of the Draw Frame(1) To straighten the fibres and to make them parallel to the central axis of the sliver. This is done by subjecting the sliver in between several pairs of rollers with each subsequent pair of rollers moving faster than the previous one. The drafting tends to reduce the linear density of the sliver.(2) To improve the evenness of the sliver. This is achieved by feeding more than one sliver at the draw frame and drawing it together. The feed of multiple slivers is called as doubling. Most commonly 6 to 8 sliver are fed to the draw frame and hence a doubling of 6 to 8 is achieved. The doubling reduces the mass variation of the sliver by averaging out the heavy and light sections of the sliver. The decrease in the linear density of the sliver caused by drafting is balanced out proportionately by combining a number of card slivers.(3) The doubling process at the draw frame in addition to improve the evenness of the silver can also be used to blend different origin of fibres. For example to obtain a 50:50 blend of cotton and polyester fibres equal number of both cotton and polyester card slivers must be doubled together provided that the count of all card slivers is same.(4) To produce a proper weight of sliver required for the following process. Doubling and drafting are the two main processes employed at the draw
67. frame. Drafting tends to decrease the linear density of the sliver whereas doubling tends to cancel out the effect of drafting. If drafting and double are of same proportion then the drawn silver will have same linear density as that of the card sliver. But if the drafting employed is more than the doubling than the resultant drawn sliver will be finer than the fed card sliver and vice versa. Therefore the degree of drafting and doubling actually depends upon the required final count of the yarn.Main Parts of the Draw FrameThe draw frames are built with one or two deliveries. The single delivery drawframe is more efficient and flexible but the double delivery draw frames have theadvantage of having twice the production covering nearly the same floor area asthat of the single delivery draw frame. The double delivery draw frames alsohave a less initial cost. A standard draw frame is divided into following sections:(1) Creel Section(2) Drafting Section(3) Sliver Condensing Section(4) Coiler Section(5) Suction Section(1) Creel SectionCreel is the portion of the draw frame where the card sliver cans are placed. Thecans behind the draw frame are placed in two most common arrangements:(i) The nested creel arrangement(ii) In-Line creel arrangementIn nested creel arrangement, the cans are placed in a rectangular group. Suchan arrangement is exclusively used for single delivery draw frames. On the otherhand the in-line creel arrangement has all the cans placed in a straight line andis mostly used for double delivery draw frames. Both the arrangements areshown below:
68. Nested Arrangement In-Line ArrangementThe sliver coming out of each can is passed over a guide plate and is fed to themain drafting rollers. The sliver is either directly pulled by the drafting rollers orin order to avoid unnecessary stretch it is pulled by power driven rollers placedjust above the cans. The creel also sometimes has an automatic stop motion todetect sliver breaks and on breaking of any sliver, the machine will be stopped.(2) Drafting SectionThe drafting of the sliver at the draw frame is carried out by roller draftingmethod in which the card sliver is passed through two or more pairs of rollers. Inmodern draw frames the top roller used are rubber coated and are called as cotswhile the bottom rollers are steel rollers having fine flutes on their surfaces. Thecots exert pressure on the bottom rollers and their surface is treated with anti-static material. The back cots exert less pressure as compared to the nextsucceeding cot in the drafting system.The surface speed of each succeeding pair of roller is kept more than theprevious one. The slower pair of roller grips the fibres whereas the next fasterpair of rollers draws the fibres forward. This increases the length of the sliverand reduces its linear density by a factor equal to the ratio of the surface speedof the fast moving roller to the surface speed of the slow moving roller. Thisratio is called as mechanical draft.The distance between the two pair of rollers is called as drafting zone. Thedistance between the nip lines of the two adjacent pair of rollers is called theroller setting. The first pair of rollers (at the feed end) is called as the backrollers and the last pair of rollers (at the delivery end) is called as the frontrollers.The roller drafting systems used on various draw frames are of many types.However every roller drafting system is named according to the number of topand bottom rollers it has. Draw frames are available with 4 over 4, 3 over 3, 4over 3, 5 over 3 and 3 over 4 roller arrangements. All of these arrangementsgive good results when set appropriately. A 4 over 4 roller drafting system isshown below:
69. The over 4 over 4 drafting system has four pair of rollers and hence has threedrafting zones namely the back zone, middle zone and the front zone. The draftgiven in the back zone is called as the break draft, the draft in the middle zone iscalled as the middle draft and the draft given at the front zone is called as themain draft. The break draft is always smaller than middle draft and the maindraft is always kept the greatest. Break Draft = V2 / V1 Middle Draft = V3 / V2 Main Draft = V4/V3The total draft is the product of the individual drafts given in all drafting zones. Total Draft = Break Draft x Middle Draft x Main Draft Total Draft = V2/V1 x V3/V2 x V4/V3 = V4/V1In addition to 4 over 4 drafting system various other drafting systems are shownbelow:Fibre Straightening During Drafting
70. As the fibres are drafted out at the draw frame, the hooked fibres are alsostraightened out. This is illustrated in below:In this example for simplicity three fibres are shown to be caught between twopair of rollers. The roller pair (A) is moving at a linear speed of 100 m/minwhereas the roller pair (B) is moving 5 times faster at 500 m/min. When theslower hooked fibre (1) held by the nip of roller pair (A) comes in contact withthe faster moving fibres (1 & 2) held by the nip of roller pair (B), the fasterfibres (1 & 2) will tend to pull the slower fibre (1) and the hooked end will bealigned with other fibres moving in the same direction.Roller SettingsThe roller setting which is the distance between the nip lines of the two adjacentpair of rollers is mainly governed by the fibre length. The roller setting is keptwidest apart in the back zone while it is narrowest in the front zone. This is dueto the fact that fibres in the back zone will have more hooks and a wider spacingmust be given in this zone to allow the fibres to attenuate and grow. Since fibresreaching the front zone will have many of their hooks removed by the previouszone so less wide roller spacing is required here.When adjusting roller settings, the distance between the nips of the twoadjacent rollers should be just wide enough to let the longest fibre grow. If thespacing is too narrow, the longer fibres will break. If the spacing is too wide thentoo many fibres will float in between the two draft zones. The floating fibres arethe ones which are not held by any pair of drafting rollers. Floating fibres canbulge at a point to create thick and thin places. The succession of thick and thinplaces along the sliver is called as the drafting wave. Drafting wave may also becaused by worn off cots and other machine imperfections.(3) Sliver Condensing SectionThe flat fibre web (consisting of several card slivers) exiting the drafting sectionmust be converted back into a web. The fibre web leaving the front pair ofdrafting rollers is passed through a converging tube and is guided to a speciallydesigned condensing funnel called as the trumpet guide as shown below:
71. The degree of condensing at the trumpet guide is essential for providing a goodfibre to fibre cohesion to hold them better in a sliver. However if too muchcondensing is done then the drawn sliver develops thick places.After condensing of fibres at the trumpet guide back into a sliver form, the sliveris passed through a pair of calender rollers which does a further compressing ofthe fibre mass and ultimately deposits the drawn sliver into a sliver can.(4) Coiler SectionThe drawn sliver coming out of the calender rollers is passed through a coilertube fixed on a coiler plate. The coiler gears fixed on the coiler plate help torotate the coiler tube so that sliver can be laid in the can in form of special coils.The can rests on the rotating plate, with the rotation of the plate the can alsorotates. The rate of rotation of the can is kept slower than the rate of rotation ofthe coiler tube. This helps in proper deposition of drawn sliver in a spiralarrangement.It is necessary to keep the sliver deposition rate slightly higher than the sliverdelivery so that blockage of the sliver in the tube may be avoided. However thisdifference should not be too large where false draft may arise in the sliver.
72. (5) Suction SectionAs the fibres move swiftly over the surface of the drafting rollers, dust and lintmay be dislodged into the air. The purpose of the suction system on the drawframe is to remove these particles so that they might not get deposited on thesurface of the drafting rollers and also to maintain a dust and lint free workingenvironment. The accumulation of the fibrous mass on the surface of the rollerscauses unevenness in drafting and sometimes also causes sliver breakagescausing the machine to stop. A typical air suction system used on the drawframe is shown below:THE ROVING PROCESSThe drawn sliver is composed of clean and straightened fibres lying parallel toone another and to the axis of the sliver. These characteristics of a drawn sliverare ideal for creation of a yarn. However this is not possible because if the drawnsliver is to be directly converted into a yarn it would require a mechanical draftof a range of 300 to 600. But even on the most modern machines technologicallyit is not possible construct a ring frame that could give such high drafts in asingle process. So an intermediate stage of drafting is carried out using theroving frame. The draft given at the roving frame reduces the linear density ofthe drawn sliver into a less thick strand of fibres suitable as an input to the ringframe. This roving which is fed to the ring frame can then be easily convertedinto a yarn by giving a draft of 15 to 40.Another advantage of making roving is to have a better package as an input tothe ring frame. The roving frame produces roving on compact small packagescalled as bobbins. The bobbins are much more convenient to transport and haveless chances to get damaged as compared to the can sliver mode of package.In earlier times because of lack of technological advancements in draftingsystems, to produce a roving three separate machines were used one afteranother. The first machine was called as the ‘Slubber’, the second machine as‘Intermediate” and the third machine as the ‘Jack Frame’. As improvements weremade in the roving frame to give higher drafts, the process of roving formationcan now be accomplished by using only one machine called as the Roving Frameor the Simplex Frame.
73. Lot of research is being carried out on the prospects of creating a yarn directlyfrom the drawn sliver eliminating roving frame. Some modified ‘sliver to yarn’ring spinning frames equipped to give mechanical draft of 600 have already beenmanufactured and are used for research purposes. In near future the rovingframe in addition to the draw frame is one more candidate that is facingelimination from the scene of the short staple spinning.Functions of The Roving Frame(1) The basic function of the roving frame is attenuation or drafting so that the mass per unit length of the sliver may be reduced down to the extent which is suitable to be fed to the ring frame. The range of draft given at the roving frame is 5 to 20.(2) After drafting the fine strand of fibres (roving) has very little coherence and becomes unsuitable for further attenuation at the ring frame. So a protective twist must be imparted to give coherence to the fibres and to give strength to the roving. The amount of twist given at the roving frame is low and ranges from 0.7 to 2 TPI.(3) The drafted and twisted roving has to be properly wound on a package called as bobbin. This is done by the winding operation at the roving frame. The winding operation is a complex mechanical process which not only winds the roving on the bobbin but also maintains a special built of the package.Main Parts of the Roving FrameA standard type of a roving frame has following sections:(1) Creel Section(2) Drafting Section
74. (3) Winding Section(1) Creel SectionThe creel is the area designated for the drawn sliver cans which are positioned atthe back of the machine. Just above the cans number of independently drivenguide rollers are provided that helps the sliver to move toward the draftingsection. Since the fibres in the drawn sliver have less coherence so it isnecessary to keep the surface speed of the guide rollers equal to the surfacespeed of the back drafting rollers so that any false drafting may be avoided thatcan damage the sliver. Just before the drafting section a photo-electric stopmotion is used which detects the presence of the sliver and as the sliver breaksit automatically stops the machine.(2) Drafting SectionA typical drafting section of the roving frame is composed of 3 over 3 rollerarrangement. However some of the machines also make use of 3 over 4 rollerdrafting arrangement. Regardless of the type of roller arrangement the bottomroller used is always a steel fluted roller while the top roller is covered with somesynthetic rubber covering. The top rollers are pressed down with sufficient forceon to the bottom rollers to ensure proper grip of the fibres. A pressure of 100 to250 N per roller is provided on the top rollers by using mostly the springpressure. However in addition to spring pressure, pneumatic and magneticweighting is also used by some manufacturers. A simple 3 over 3 roller draftingarrangement is shown below:In the modern roving frames a double apron system is provided at the middlepair of drafting rollers. The top apron is short while the bottom apron is longer.Both of these aprons are made of either soft leather or synthetic rubber. Boththese aprons in cooperation with each other guide and transport the fibresduring drafting. The aprons help to support the floating fibres and drasticallyreduce the drafting wave. It is important that the aprons should extend as closeas possible to the nip line of the front rollers. The length of the aprons alsocalled as the cradle length is kept approximately equal to the staple length of thefibres.Use of Condensers in the Drafting SectionThree specially designed trumpet guides or condensers are used in the draftingsection of the machine. First trumpet guide also known as in-feed condenser isused just before the back pair of drafting rollers and its purpose is to lead the
75. sliver properly into the drafting arrangement. The second trumpet guide is usednear the nip of the middle pair of rollers and the third one is used just before thefront pair of rollers. The main function of the last two guides is to bring back thefibre mass into a strand that tends to tear apart because of the drafting action.The trumpet guides are usually mounted on a reciprocating bar giving the slivera traversing motion so that the wear of the rollers may spread out graduallyover the entire width of the roller.Draft DistributionAn important consideration of the drafting zone is the draft distribution i.e. howmuch draft should be given in the back and front zones. The draft at the backzone is called as break draft and it should be as low as feasible while majority ofthe draft is given at the front zone where there is an apron control over thefibres and is called as the main draft. The total draft is the product of break andmain draft. Generally the break draft for cotton lies in the range of 1.05 to 1.15and all the remaining draft is given at the main drafting zone. The break draft isjust meant to straighten the fibres and to prepare them for a major draft at thefront drafting zone. If the break draft is increased beyond an optimum valuethen the evenness of the spun yarn drastically reduces due to the formation ofthick and thin places.(3) Winding SectionThe winding section comprises of a spindle and a flyer. A spindle is a long steelshaft that acts as a support and a driving element for the flyer. The flyer is aspecial component of the roving frame that helps to insert twist in the roving.The spindle is mounted at its lower end in a bearing which gets its drive from thetrain of gears and transmits it to the flyer. Just around the flyer a shaft is fixedaround the spindle with a collar that gets its drive independently from a separateset of gears. An empty hollow package made of wood or plastic is mounted onthis shaft. The arrangement of a spindle and a flyer is shown below:
76. The winding portion of the machine with the help of the spindle and the flyermeets the following two main objectives of the roving frame:(1) Twisting(2) Package Winding(1) TwistingThe sliver after being drafting out to form a roving coming from the frontdelivery rollers have little fibre cohesion among themselves and is weak to bewound on packages and also may not sustain further drafting at the next stageof processing i.e. the ring frame. So in order to give cohesion and strength tothe roving strand a small amount of protective twist is given. The twist isimparted by using a flyer method of twist insertion.The roving coming out of the front delivery roller is threaded through the top ofthe flyer, passes through its hollow leg around the presser arm on to the bobbin.The presser arm maintains certain tension on the roving which is necessary forproper compact winding.The flyer rotates with the spindle at a constant speed with each revolution of theflyer inserting one twist in the roving strand. The relation is given by:
77. Twist Per Inch = Flyer Rotary speed (rpm)/ Delivery Speed (inches/min)Since the rotary speed of the flyer is constant so the amount of twist insertedper unit length depends upon the delivery rate of the front delivery rollers. Highvalues of twist cause production loss along with difficulty in drafting at the ringframe. On the other hand very low twist makes the roving weak and it can breakduring the package winding. The level of twist inserted for cotton at the rovingframe is about 0.7 to 2 TPI.(2) Package WindingIn order for the winding to take place on the surface of the bobbin, the surfacespeed of the roving coming from the flyer should be different from the surfacespeed of the bobbin. The bobbin therefore is driven independently of the flyerand it rotates with the collar around the spindle. Winding at the roving frame ispossible by one of the following two methods:(1) Bobbin Lead Method(2) Flyer Lead Method.In the bobbin lead method to facilitate winding, the surface speed of the bobbinis kept greater than the surface speed of the flyer. On the other hand in flyerlead method, the surface speed of flyer is kept more than that of the bobbin. Incotton roving frame, the bobbin lead method is used.The Package BuiltThe roving coming out of the hollow leg of the flyer is made to wind on acylindrical package called as the bobbin. The bobbin is either made of wood orplastic. The roving is wound on the bobbin in such a way so that tapered ends onboth sides of the package are formed. The angle of taper of the ends liesbetween 80° to 95° depending upon the adherence of the material. Byincreasing the angle of taper, larger packages are possible to make however theadherence between the layers decreases. On the other hand low angle of tapergives better adherence to the material but only smaller packages are possible tomake with it.
78. Bobbin is an ideal form of a supply package to be fed to the ring spinning framebecause when full it can hold large length of roving owing to its compactnessand when empty it is light and occupies small volume and is easy to handle andtransport.The Builder MotionThe above mentioned required package built is not easy to construct. There arelots of complex mechanical arrangements provided at the roving frame toachieve this. Due to these special winding needs at the roving frame it makes ita very complicated machine. The builder motion is a device or series ofmechanical arrangements necessary to obtain a proper built of the rovingbobbin. The builder motion performs the following important tasks related to thepackage built:(1) Controlling Bobbin Drive(2) Controlling Lifter Motion of Bobbin Rail(3) Formation of tapered ends(1) Controlling Bobbin DriveDuring package winding with each new layer of roving wound on the bobbin, thediameter of the bobbin increases which causes the surface speed of the bobbinto increase as well. However for a uniform package winding, it is absolutelyessential to keep the difference in the surface speed of the flyer and bobbinconstant. Since the rotary speed of flyer in a roving frame is kept constant so tokeep this difference of the surface speed constant, the rotary speed of thebobbin is reduced proportionately with the increase in its diameter.The reduction in the rotary speed of the bobbin originates from a cone drumdrive. With each new layer of roving wound on the bobbin, the builder motion
79. shifts the cone belt enough to reduce the rotary speed of the bobbin so that itssurface speed may remain constant A simple arrangement of a cone drum driveis shown in the figure below:(2) Controlling Lifter Motion of Bobbin RailThe roving package is created by placing layer upon layer of parallel coils ofroving on the surface of the bobbin. The built of the package is carried out in aprecision manner where each successive layer or coil of roving is laid in a precisespacing to the previous coil. This can be achieved by(i) Raising and lowering of the flyer.(ii) Raising and lowering of the bobbinThe flyer is never moved because by doing so the unsupported length of theroving coming from the front delivery roller to the top of the flyer will vary. Alsothe angle of the roving from the front delivery roller to the flyer top will alsochange. This can cause uneven winding tension and is not suitable. So the onlyway to achieve a proper built of the package is to move the bobbin up and down.For this purpose the bobbins are supported by a movable rail that lifts andlowers the bobbins as per requirement.
80. Since the package diameter is steadily increasing, the lift speed must also bereduced by a small amount after the completion of every layer. This is necessarybecause with a bigger diameter of the package more length of roving will beaccommodated and the lifting and lowering of the bobbin should be sloweddown. To obtain this, the drive to the lifter mechanism is also obtained from thesame cone drum drive used for the bobbin.The lifter mechanism is also fitted with a reversing mechanism so that thebobbin rail is alternately raised and lowered so that the roving could be woundon the entire length of the bobbin.(3) Formation of Tapered EndsIn order to form a special taper ends on the bobbin the height of the lift throughwhich the lifter motion is going to raise and lower the bobbin is graduallyreduced after each layer of roving has been completed. For this the buildermotion of the roving frame is fitted wit special micro switches that perform thisaction.Controlling the Roving TensionThe roving coming out of the lower end of the hollow leg of the flyer passes overa presser arm. The presser arm has to guide the roving from the lower exit ofthe flyer leg on to the package. Before the roving could be wound on thepackage it is wrapped two or three times on the presser arm.
81. Two Turns on the Arm Three Turns on the ArmThe number of turns determines the roving tension. More turns would meangreater roving tension and would result in a harder and more compact rovingpackage. However the tension should not be kept so high where false drafts orroving breakages may occur.THE RING SPINNING PROCESSThe ring spinning is the final operation in the formation of the ring spun yarn.The basic purpose of the ring spinning frame is to attenuate the roving until therequired fineness of the yarn is achieved. The ring spinning machine was firstinvented in 1828 in America. Since then a lot of modern modifications have beencarried out but the basic principle of operation and the basic machine design
82. remains the same. Even with the introduction to new sophisticated spinningsystems, the ring spinning system is widely used and is the most popular form ofspinning system. The reason behind is the ability of this system to produce veryfine yarns which is not possible to obtain at the moment with any other form ofspinning systems. Only the rotor spinning system provides good competition tothe ring spinning system which again can not produce fine yarns of the orderproduced by the ring spinning frame.The initial and maintenance cost of the ring spinning is quite high. The ringframe contributes about 60% towards the final cost of production of the yarn. Soevery effort is being put in to make modify the ring spinning machine to givemore productivity at a less cost.Functions of The Ring Spinning Frame(1) The basic function of the ring spinning frame is drafting. Drafting is carried out to such an extent so as to achieve desired fineness of the yarn. The drafting is carried out by using a 3 over 3 roller drafting arrangement with double apron support. At the ring spinning frame a draft of 15 to 40 is given (sometimes also up to 50).(2) The attenuated yarn formed by drafting is weak and lack cohesion. In order to give strength to the final yarn, twist is inserted. Twist is inserted at the ring spinning frame by using the popular traveller method. The amount of twist inserted in the yarn varies with the count of the yarn. To make finer yarns, greater TPI is given and vice versa. The value of Twist Multiplier (TM) at the ring spinning frame generally ranges from 3 to 5.(3) The final yarn produced after drafting and twisting is wound on special ring bobbins also called as cops. The built of the package kept is such which is suitable for storage, transportation and further processing.Main Parts of The Ring Spinning FrameThe ring spinning frames are double sided or double delivery machines havingup to 500 delivery points or spindles on each side. Hence a single machine canhave a capacity of up to 1000 spindles.A typical ring spinning frame is divided into four zones:(1) Creel Zone(2) Drafting Zone(3) Twisting Zone(4) Package Winding Zone
83. (1) Roving Bobbin (2) Roving (3) Bobbin Holder (4) Guide Rail (5) Drafting Arrangement (6) Yarn (7) Yarn Guide (8) Spindle (9) Traveller (10)Ring(1) Creel ZoneThe creel of the ring spinning frame is a simple device that holds the roving. It isvery important that the roving should unwind properly and evenly to avoid anyfalse drafts or roving breakages. To facilitate proper unwinding the rovingbobbins are held vertically by inserting the roving bobbin on the bobbin holderplaced at the upper portion of the frame. A typical bobbin holder is shown in thefigure below:
84. Ring Retainer DeviceThe upper end of the bobbin holder is suspended by a bearing. The rovingbobbin is pushed upward on to the bobbin holder. Since the ring of the bobbinholder is attached to the retainer device so as the bobbin is pushed upward, thering will also move upward causing the retainer device to grab the inner portionof the roving bobbin tube.As the roving is pulled forward by the drafting rollers, the roving bobbin rotatesand unwinding takes place. To avoid excessive rotation to the bobbin, a brakearm is used to lightly press the roving bobbin to restrict its motion. Alternatelythis can also be achieved by using internal brakes in the ball bearings.(2) Drafting ZoneSince the at the ring spinning frame greatest value of draft is given, the draftingzone of the ring frame is the most important part of the machine that directlyinfluences the evenness and strength of the yarn. So it is important to have aprecision control on the fibres in the strand which is being drafted out tosuppress the drafting waves. Pendulum Arm for Weighting
85. All the modern ring spinning frame makes use of a 3 over 3 roller drafting withboth the top and bottom middle rollers covered with aprons. The bottom rollersare steel fluted and are driven positively. The top rollers are covered withsynthetic rubber coating and are driven by the frictional contact with the bottomrollers and are hence pressed down on the bottom rollers with a considerableforce. For this purpose the top rollers are weighted by using spring, pneumaticor magnetic weighting with the help of a pendulum arm.A total draft of 15 to 40 and in some cases even up to 50 can be given at thering spinning frame. The distribution of draft in the back and front drafting zoneis very important as a proper draft distribution helps to reduce the drafting waveproblem. Practically the break drafts should be given in the range of 1.1 to 1.5and the remaining draft is given in the main drafting zone. High degree ofdrafting in the front zone will tend to create drafting waves. To avoid this middlepair of drafting rollers is covered with aprons. Aprons give support to the fibresthrough out the roller spacing between middle to front rollers not letting eventhe shortest fibre to float. Apron systems are not perfect but they help todrastically reduce drafting waves. Based upon the type of the bottom apronused, two types of apron systems are used commercially on the ring spinningframe:(i) Short Bottom Apron System(ii) Long Bottom Apron System Long Bottom Short Bottom Apron System Apron SystemThe short bottom apron system was used in old machinery. Although the shortaprons require a simpler design of the ring frame and also have the advantagethat they can be brought more close to the nip of the front rollers, however theyare difficult to replace when damaged and can also cause choking of fibre mass.To avoid these limitations the modern spinning machines make use of longbottom aprons..Using Trumpet GuidesThe strand of roving has few numbers of fibres in a cross-section and upondrafting even fewer number of fibres will remain in a yarn. These fibres havehardly any cohesion between themselves. Special fibre guiding elements aretherefore essential to carry out drafting without breaking the strand. For thispurpose specially designed trumpet guides are used in the drafting zone to helpkeep the fibre mass together and to avoid tearing apart of the strand. Threetrumpet guides or condensers are used one just before the back pair of rollers,second in between the back and middle rollers and the last just before the frontpair of rollers. These guides are mounted on reciprocating bar that oscillates
86. slowly so that the wear of the rollers may spread out gradually through out theentire roller width.Overhang of Front and Middle Top RollerAs the twist is given to the yarn with the help of a traveller, the twist must runback as close as possible to the nip line of the front rollers. But it neverpenetrates completely to the nip because at the nip the fibres are divertedinwards and are made to wrap around the surface of the roller. So at the exitpoint of the front pair of rollers there is always a small triangular mass of fibreswhich remain without twist, this is called as the spinning triangle. This trianglebundle of fibres will remain without twist during twisting and create a weak pointin the yarn and hence breakage rate of the yarn during spinning increases. Theeffect of spinning triangle is enhanced at the ring spinning frame where greatestdraft along with greatest twist is applied. Top Front Roller Spinning Triangle Bottom Front RollerSo in the ring spinning drafting arrangement the front top roller is deliberatelykept 2-4 mm forward relative to the bottom front roller while the middle toproller is kept 2-4 mm backward relative to the middle bottom roller. This type ofarrangement gives smooth running of the top roller and helps to reduce spinningtriangle and ultimately the breakage rate during the spinning process is reduced.
87. To further enhance the flow of the fibre strand through the draftingarrangement, the drafting roller instead of being placed in a straight horizontalline as depicted from the above figure, they are arranged at certain inclination.(3) Twisting ZoneThe yarn leaving the front pair of drafting rollers is threaded through a guidealso called as the lappet guide that is placed directly over the spindle axis. Theyarn then passes through a traveller on to the yarn package (cop). The travelleris mounted on the ring encircling the spindle. The cop is mounted on the spindleand rotates with the spindle. When the cop rotates the tension on the yarn pullsthe traveller to rotate around the ring. Due to the friction created between thetraveller and the ring and also due to the air drag created by the balloonformation at the winding section, the rotary and surface speed of the traveller isslightly less than that of the spindle and is given by: RPM of Traveller =RPM of Spindle – Delivery Speed / π x Package DiaSo in one rotation of the traveller one twist is inserted in the yarn. Since thedifference between traveller and spindle rotary speed is very small so thisdifference is ignored. Thus for calculating twist rotary speed of the spindle isconsidered, mathematically: T.P.I = Rotary Speed of Spindle (rpm) / Delivery Speed (inches/min)The ring/traveller arrangement and the spindle are also very important elementsof the ring spinning frame because it not only helps to insert twist in the yarnbut also helps in the winding of the package. Lappet Guide Cop Separator Traveller Ring Rail Ring Spindle Belt Drive
88. The RingThe rings are supported on the raisable and lowerable ring rail. The ring shouldhave a tough, hard and smooth surface. For this purpose flame hardened steel,nitrided steel, carbo-nitrided steel and chrome steel is used. The hardness of thetraveller should be less than that of the ring so that wear mainly occurs on thetraveller which is cheaper and easier to replace.The rings can either be classified as:(i) Lubricated Rings(ii) Un-lubricated RingsLubricated ring is used for woollen and worsted spinning where externallubrication on its surface is applied. For cotton and other short staple spinningonly un-lubricated rings are used. This is due to the fact that that all naturalshort staple fibres are made up of cellulose and has small quantity of naturalwaxes in it. As the yarn moves swiftly with the traveller, a lubricated layer ofwaxes and cellulose is generated due to the abrasion of the fibres. Thislubrication is beneficial for decreasing the friction between the traveller and thering and ensures a smooth continuous running. The amount of lubricationgenerated depends mainly upon the count of the yarn spun and quality of rawmaterial being used. Coarser yarns generally produce more lubrication.On the basis of working sides of the ring, rings can also be classified as:(i) Single Sided Rings(ii) Double Sided Rings.Double sided rings have the advantage of having two working sides. When oneside gets abraded the ring can be turned over so that the other side can beused. Whereas when single sided rings get damaged, they have to be replacedby new ones. However double sided rings are not used anymore because when itis time for the ring to be turned over, the other side of the ring will becomeunstable due to corrosion and rusting and can not be used.The TravellerThe traveller is an important element of the ring frame as it imparts twist on theyarn and also helps in winding the yarn on the cop. The traveller does not havea drive of its own but is dragged along with the yarn as it gets wound on the copdue to the rotating spindle. As the traveller moves at a high speed on the ring itcreates lot of friction that generates significant amount of heat. So in order tocope up with such frictional forces the material used for traveller should exhibitthe following properties:(i) Generate as little heat as possible.(ii) Should dissipate heat quickly to the ring and the air.(iii) Should be elastic so that it might not break.(iv) Should have high wear resistance.(v) Should have less hardness than the ring.To meet these requirements, the traveller is made exclusively of steel having itssurface either electroplated with nickel and silver or treated with chemicals toincrease wear and reduce friction.
89. Different types and varieties of yarns can not be spun using a single type oftraveller. Therefore travellers come in many different varieties. The differencesamong travellers are found in shape, mass, wire profile and yarn clearance (bowheight). Flat Traveller C-Traveller N-Traveller Elliptical TravellerThe traveller is shaped according to the ring so that single point of contact withgreatest possible surface area with the ring can be achieved. The height or bowof the traveller should be as low as possible to keep the centre of gravity lowand to ensure smooth running. However the bow should be not so small wherethe yarn starts getting abraded which can damage the yarn hairiness.Another important parameter of the traveller is its mass. The mass of thetraveller directly influences the frictional forces between itself and the ring. Themass of the traveller is selected according to the yarn count being spun. If thetraveller is too light for a specific yarn count then tension created on the yarnwill be low resulting in a loose softly wound cop and also the size of the balloonincreases. On the other hand, if the traveller is too heavy then it causesexcessive tension on the yarn and cause frequent yarn breakages. Forconvenience instead of the traveller weight they are standardized by its number.The following table shows various traveller numbers suitable for different yarncounts: Yarn Traveller Number For Traveller Number For Count Cotton Synthetics and Blends 85 16 22.4 75 20 28 65 23.6 31.5 60 26 35.5 50 31.5 40 42 35.5 45 35 45 56 30 56 71 24 71 90 20 90 100 16 100 112
90. Limitations of Traveller/Ring ArrangementThe greatest limitation faced by ring spinning frame is its incapability to furtherincrease its productivity and speed. This is mainly due to the use of traveller ringarrangement. At high speeds the traveller generates significant amount of heatdue to friction with the ring. If the speed of the ring frame is to further increase,owing to a very small mass and size of the traveller, dissipation of heatgenerated by the traveller is not possible. Thus the operating speed of thetraveller and the ultimately the entire machine is limited. Currently the spindle ofthe ring frame is capable of running up to 30,000 rpm but the use of travellerpermits the speed only to be raised up to around 22,000 rpm.Another way of increasing the speed of the ring frame is by using ring withsmaller diameter so that spindle speed can be further increased withoutincreasing the frictional forces on the traveller/ring. However by doing so smallerpackages will be formed and they will have to be doffed more frequently. Thiscan decrease the productivity of the machine. However this problem can berectified by using automatic doffing devices.To put into a nutshell, there is a very small room as far the speed advancementin the ring spinning frame is concerned. However measures like automaticdoffing, use of precision instruments and precision components (specially ringand traveller), increase in the number of spindles per machine to reduce cost perspindle and automatic linkage of ring frame with the winding machines will helpthe ring spinning frame to be economically viable to use for years to come.(4) Package Winding ZoneThe yarn after being twisted by the traveller has to be properly wound on theentire length of the package called as the cop. In order for the winding to takeplace there should be a difference in the surface speed between the spindle andthe traveller. The traveller has no drive of its own instead it is carried along withthe yarn which is being wound on the cop after passing through the traveller.The frictional forces between the spindle and the traveller and also the air dragbecause of the balloon formation between the lappet guide and the spindlemakes the surface speed of the traveller less than that of the spindle. Thisautomatically fulfils the requirement of winding. The traveller and the spindlecooperate with each other to perform winding.In order for the yarn to be properly wound on the entire length of the cylindricalring bobbin (cop), the ring is raised and lowered which is mounted on alongitudinal ring rail.The SpindleSpindle is a very important component of the ring frame, it not only supports thecop and helps in winding of the yarn on it but also gives motion to the traveller.The spindle and the traveller therefore work in close cooperation with each otherto perform both twisting and winding.A spindle is a metallic shaft that holds the yarn package or cop. The spindle isdivided into two main parts namely the upper part and the bolster.
91. Upper Tapered Part Ring Rail BolsterThe upper part is made of aluminium alloy and is slightly tapered to firmly holdthe package. The bolster or the lower part is secured in a bearing to rotate freelyand is also connected to the ring rail by means of a nut. The drive to the spindlecan either be given with the help of tapes or belts in group form or in individualform where one motor is supplied per spindle.Package Built of Ring Spinning FrameA typical form of a package produced by a ring spinning frame is called as thecop. The package is produced on a tube of paper, card board or plastic material.About 10 mm of the tube is left free of the yarn on both upper and lower ends.The tube has a slight taper corresponding to the taper of the spindle so that thepackage can be firmly secured on the spindle. Upper Cross Winding Conical Tip Layers Middle Cylindrical Part Main Winding Layers Lower Curved Base Package Tube
92. The structure of the cop is divided into three distinct parts:(1) The Upper Conical Tip.(2) The Middle Cylindrical Part.(3) The Lower Curved Base.The cop has two distinct layers of the yarn wound on its surface i.e. the mainwinding layers and the cross winding layers. The main winding layers are closeto each other and are densely wound whereas the cross winding layers areopenly laid and are loosely wound. The cross winding layers separates the mainwinding layers so that the high tension of the yarn may not cause the successivelayers to be pressed causing problems in unwinding. The package built of thecop as compared to that of the roving bobbin is much more complex which alsorequires complex mechanical arrangements; however it is optimal for unwindingat a very high speed on the winding machines.The Builder MotionTo obtain the above mentioned built of the cop, complex mechanicalarrangements called as the builder motion is provided at the ring frame. Thebuilder motion achieves the structure of the cop by performing the followingtasks:(1) The ring rail on which the ring is mounted is moved up and down by the builder motion in a special manner. The ring rail while moving up is moved slowly but with an increasing speed and is moved down quite faster but with a decreasing speed. During the slow upward movement of the ring rail, a dense main winding layer is laid and during the fast downward movement, a loose cross winding layer is laid. This gives the ratio between the length of the yarn in the main and cross windings to be 2:1. This difference in yarn length in the upper and middle part creates a taper or conical shape of the upper part. The stroke or the distance by which the ring rail moves up and down is less than the total winding height (lift) of the tube.(2) The stroke of the ring rail is deliberately kept less than package tube height so that the ring rail can be moved upward by a small distance from the previous point of lay of the yarn after one complete layer of the yarn has been laid. This helps in creating the lower curved base of the package. In older machinery, instead of moving the point of lay of the ring rail upwards after every layer has been laid, the spindle is made to move downward. This is carried out by mounting the spindle on the spindle rail. However in modern machinery this arrangement is no longer used and only the ring rail is made to move up and down and also its point of lay is continuously lifted upwards by a small amount. This somehow reduces the complexity of the builder motion.The tasks of the builder motion to move the ring rail up and down is carried outby using special heart shaped eccentrics or cams in its drive given to the ringrail. These eccentrics in its rotary motion give an up and down motion to the ringrail. The rise in the point of lay of the ring originates by using a ratchet wheelthat after every layer of the yarn makes the pint of the lay of the ring rail to shiftupwards.
93. Use of Balloon Control Rings (BCR)To achieve greater production speeds with minimum friction produced by thetraveller, the spindle and the rings used on modern ring frames arecomparatively small. This small ring size only permits a very limited length ofyarn to be wound on the bobbin and the doffing would have to be performedmore frequently and hence the productivity would suffer. On modern machinesthis problem has been over come by using longer length of spindles and bobbinsso that even with less package diameter more yarn length can be wound. Thisreduces the amount of doffing and productivity can be increased in this way.The use of long spindles will mean that the distance between the lappet guideand the ring would be quite high resulting in a formation of a bigger balloon. Thegreater balloon size has following disadvantages:(i) To facilitate a larger balloon during winding, more spacing will be required between the adjacent spindles and hence the size of the machine has to be increased.(ii) The large balloon causes the air drag on the yarn to increase and due to which the yarn can be broken due to balloon collapse.In order to avoid these disadvantageous effects, balloon control rings are used.Each balloon control ring divides the balloon into two smaller sub balloons whichare more stable and create less air drag on the yarn. The use of balloon controlrings is illustrated below: SubSeparator Balloons BCRs
94. The balloon control rings enable the spinning operation with long spindles at highspeeds. However the use of such rings cause the surface of the yarn to becomerough and abraded as the yarn is rubbed against the surface of these rings. Thiscan also creates more fly in the spinning department.Use of SeparatorsMost of the end breakages during spinning occur because of the weak spotscreated by the spinning triangle. When the thread breaks the free broken end ofthe thread lashes around the spindle. If a protective plates called as separatorsare not provided to separate the adjacent spindles, the broken end of the threadcan get entangled into the neighbouring spindles causing more threads to break.So a single end breakage can cause a chain reaction of yarn breakages in all thespindles placed in one line. To prevent this separator plates made up ofaluminium or plastic is placed in between every adjacent spindle.
95. THE WINDING & CLEARING PROCESSThe quantity of yarn on the ring spinning bobbins or cops is very small ascompared to the size of the package required for efficient processing at theknitting and weaving process. In addition to the small package size, the ringbobbins are also full of spinning defects i.e. thick and thin places.So the process of winding involves unwinding of the yarn from the spinningpackages i.e. ring bobbins and winding it on to a new bigger package. During theformation of the new package, spinning faults i.e. thick and thin places are alsoremoved. Two types of packages can be produced by winding machine i.e.cheeses or spools (rectangular or parallel side packages) and cones (taperedside packages). But the type of package build within these two types ofpackages can vary depending upon the end use of the package.It appears that winding process is just a simple process where the yarn isunwound from the ring bobbins and again wound on the new package and itseems that winding has no great significance but this is in fact not true. Supposeif we use ring bobbins directly in the process of weaving or knitting, thenfollowing problems may arise :-(1)The ring bobbins will keep on exhausting very quickly and lot of time will be wasted in replacing the empty bobbins with new ones.(2) The ultimate fabric produced by using ring bobbins will have defects and a lot of time and resources will go wasted.(3) Because of the thin places in the yarn, threads will break more frequently during the fabric formation and thus efficiency and production will suffer.All these points make the winding process very important. Even though it is anextra and expensive process for the preparation of a suitable package for fabricformation but still it proves its worth.Objectives of Winding Process(1) To prepare a bigger package having a sufficient length of yarn on it.(2) To remove spinning faults e.g. tick and thin places.(3) To improve the quality of yarn.(4) In some cases, the yarn is also treated with certain chemicals or dyes during the winding process. Waxes are also applied to the yarn to reduce the abrasion and friction during the winding process.(5) To produce a package of required density and shape suitable for the next stage of processing.Types of Winding PackagesTwo types of packages can be produced by winding machines:-(1) Rectangular or Parallel Side Package.(2) Tapered Side Package.(1) Rectangular or Parallel Side PackageRectangular or Parallel side packages are called as cheeses or spools. Cheeses orspools are produced by slow conventional type of machines.
96. Taper Spool With Flanges Cheese Without FlangesParallel side packages are also suitable for staple fibres and for those yarnswhere the desirable length on the package is not very long. This type of packageis also suitable when the package has to be dyed. The Parallel or rectangularside packages may or may not have flanges.(2) Tapered Side PackageThe tapered side packages are called as cones. Cones are produced by highspeed winding machines like the autoconer.Many types of cones are used in the industry. Various cones differ from eachother from their package build and angle of taper. Most popular cones with theirpackage built are given below:Low Angled Taper Wider Angle Taper Wide Angle Taper Pineapple Cone(i) Low angled taper cones having a taper of 2° 20’ to 3° 30’ are used for staple yarns where long lengths of yarn is required on the package. Such cones are very suitable for high speed winding and high speed warping machines.(ii) Wider taper cones having a taper of 4° 20’ are used when the cones are to be dyed by using pressure dyeing.(iii) Wide angles cones having a taper of 9° 15’ are used mainly for the supply of the weft knitting yarn(iv) Pineapple cones have a taper of 3° 30’ just like low angled tapered cones, but their build is entirely different. These cones are produced by reducing the length of the yarn traverse as the package diameter increases.
97. Based upon the type of these winding packages produced by the windingmachines, winders are classified as:(1) Cheese or Spool Winders(2) Cone WindersWhether the winding machine is old conventional type or is modern type, thebasic principle of all the machines are same. If the winding machine producesend product as a cone (tapered side package) then it is called as cone winderand if its end product is a cheese or spool (rectangular side package) then it iscalled as cheese winder or spool winder.Components of Winding MachineThe old conventional winders are quite simple machines where majority of thenecessary mechanisms being of mechanical type. On the other hand, themodern automatic winding machines are equipped with variety of electronicdevices and computerized control panels to achieve high speeds of winding at abetter quality. Furthermore arrangement of automatic bobbin creeling, automaticdoffing and auto joining of the broken threads are also provided on thesemodern winders. Illustration of a high speed winding machine is given below: (1) Balloon Controller (2) Yarn Guide (3) Pre-Clearer Guide (4) Yarn Tensioner (5) Splicer (6) Electronic Clearer (7) Cutting Device (8) Waxing Unit (9) Yarn Trap (10) Grooved Drum
98. Typically a modern high speed winding machine is divided into following zones:(1) Creel Zone(2) Tension Zone(3) Clearing Zone(4) Yarn Joining Zone(5) Winding Zone(1) Creel ZoneCreel is the part on which ring bobbins are held. The creel is so designed so thatit should assist in continuous uniform unwinding of the yarn at high machinespeeds which in case of modern winders can go up to 1500 metres per minute.Each creel also has some sort of balloon controller which is made up of metaland does not allow bigger balloons to get formed during unwinding. Theunwinding of the yarn from the package is called as the withdrawal of the yarnor package. Two techniques might be used for withdrawal of the package :-(i) Side End Withdrawal.(ii) Over End Withdrawal.(i) Side End WithdrawalIn this method, the package is mounted on a spindle and the yarn is removedfrom its side.As long as the yarn is being removed, the package revolves. It is only suitablefor slow speed machines because at high speed, the package wobbles that cancause the tension to increase. This method is associated with rectangular orparallel packages i.e. cheeses or spools.(ii) Over End WithdrawalIn this method, the package is kept stationary and the yarn is removed from thetop. This method is suitable for high speed machines. This type of withdrawal ismostly associated with tapered side packages i.e. cones. The taper in conesusually are given to assist easy withdrawal of the yarn.
99. (2) Tension ZoneTension zone performs the following two main objectives:(i) To apply a uniform tension on the yarn so that uniform package with required density can be obtained. Greater the tension on the yarn, more compact and dense package can be obtained. However the amount of tension to be applied on the yarn depends upon the count.(ii) The tension on the yarn helps to remove thin or weak places in the yarn. To remove thin places, a sufficient tension for a certain count of yarn is applied uniformly. This tension will cause the thin or weak places in the yarn to break however the regular yarn will not be affected. In this way, these faults are removed. The amount of tension applied should be about 10 to 15% of the single yarn strength.The tension on the yarn is applied by passing it through a tensioning device ortensioner. Tensioners come in variety of shapes and techniques howeverconventionally a disc type tensioner is used in which the yarn is passed throughtwo disc plates and a sufficient pressure is applied to the plates. The amount oftension produced in this case would be directly proportional to the amount ofpressure on the discs. In modern winder more sophisticated yarn tensioningdevice is used which is controlled electronically through a computer controlpanel.(3) Clearing ZoneThe purpose of the clearing zone is to eliminate yarn defects such as thickplaces, thin places and slubs. In old winding machinery mechanical clearers areused. These clearers or slub removers are composed of fixed blade with verylittle distance left for the yarn to pass beneath or over it. As a thick place or slubcomes, the blade cuts it off the surface of the yarn. Mechanical clearers areeither flat blade or ring blade type as shown below:Mechanical clearers are very difficult to adjust; they are not reliable and durableand make the yarn surface harsh and hairy. Due to these limitations they are nolonger used on modern winder. Instead electronic clearers are used. Theelectronic clearers either work on optical or capacitance principles. Theseclearers are very efficient, reliable and durable as compared to mechanical typeand even the slightest of variation can be detected and removed by them whichis not possible in mechanical type.When optical principle is used then we use photoelectric cells. A light source isgenerated by the emitter or the transmitter and is passed through the yarn andreceived on the other end by the receiver. The amount of light received afterpassing through the yarn is translated into an electric current. For example, forcoarse yarn less light and for fine yarn more light will be received. The Electronicclearer is set for a particular count of yarn and if any slub or thin place comes onthe yarn, it is detected by variation in the light and hence it is removed by thecutter.
100. In case of capacitance type electronic clearer, the yarn is passed over acapacitance device which constantly measures the capacitance of the yarn andtranslates that capacitance into an electric current. The capacitance of the yarndepends upon the moisture in the yarn which in turn depends upon the numberof fibres in a cross-section i.e. for fine yarns, capacitance will be low and forcoarse yarns it will be high. The clearer is set according to the count, when anyvariation in capacitance that exceeds a certain limit is detected, the cutter cutsthe thread and in this way both slubs and thin places are removed.(4) Yarn Joining ZoneDuring the winding process, breakage of threads may take place. The breakageof threads may occur due to:(1) The deliberate action of the mechanical type tensioner for removal of thin places.(2) The deliberate action of the electronic clearer for the removal of thick and thin places.(3) The result of extra force build-up on the yarn due to many reasons like friction, ballooning effect, etc.As the yarn breaks, the stop motion installed on the machine causes themachine to stop immediately. In conventional winders, mechanical type stopmotion is used where the yarn is passed through a lever which is lifted due tothe tension in the yarn. As the yarn breaks the lever falls down whichmechanically or electrically stops the machine.The modern winders make use of optical sensors for stop motion. The yarn ispassed through a pair of sensor having a transmitter and a receiver. Thetransmitter transmits light which can only be received by the receiver whenthere is no yarn between them i.e. when the yarn breaks. As soon as thereceiver starts receiving the light, the machine is stopped immediately.Piecing or Joining of Broken Threads
101. Whether the yarn is deliberately cut due to the action of clearer or it accidentallybreaks, the stop motion installed on the machine will immediately stop winding.As soon as the machine is stopped, the two broken ends of the yarn must bepieced or joined together as soon as possible so that the machine can beimmediately started again. The piecing of the broken ends can be carried out byfollowing methods:(a) Knotting(b) Splicing(a) KnottingIn this method, the two broken ends of the yarn are knotted together by aregular knot. The knotting of the threads may be carried out manually by handor by automatic knotting machines. One or more than one automatic knottersmay be used per winding machine. It is always desirable to use each separateknotter or each spindle, but this increases the machine cost considerably. So thegeneral practice is to use one knotter for 10-12 spindles. The knotter will moveor patrol these spindles in a reciprocating manner and whenever it finds anyspindle stopped, it repairs the broken ends by knotting. Sometimes, only oneknotter is used for the whole machine. In this case, the knotter can eitherreciprocate between the spindles or it can move continuously in a loop aroundthe machine covering all the spindles.The method of knotting is considered to be an old method and it has manydrawbacks:(i) The presence of knot in the yarn will increase its diameter at the point of a knot. This increase may be 3-4 times the actual yarn diameter.(ii) The knot sometimes makes it difficult to pass the threads through various components of loom and needles of knitting machine.(iii) Knots can be clearly visible in the fabric degrading its quality.(iv) These knots also reduce the life of knitting needles and loom components through which the yarn is passed.(b) SplicingSplicing is a modern method of joining the broken ends. The machinecomponent that does splicing is called as the splicer. The procedure of splicing isas follows:(i) Both broken ends of the thread are collected by splicer arms by means of air suction.(ii) Each broken end is untwisted by applying twist in the opposite direction to the twist in the yarn.(iii) Both broken ends of the yarn are placed on each other.(iv) They are joined together by twisting and slight stretching.The use of splicing has many advantages over the knotting:
102. (i) The diameter of the spliced yarn does not increase more than 25% of the actual diameter.(ii) The splices in the yarn are less visible in both the yarn itself and the fabric made out of that yarn.(iii) The spliced yarn can easily pass knitting needles and loom components without damaging or increasing the wear of these components.The most efficient system would have one splicer per spindle. Such arrangementwill make the cost of the winding machine very high and also the cost ofmaintenance will increase. It is a general practice to have one splicer for smallgroup of spindles e.g. one splicer for 10-12 spindles. Either the spindles movetowards the splicer or the splicer moves towards the spindles. Commonly thesplicer moves in a circular path or in a straight reciprocating path covering thespecific number of spindles.(5) Winding ZoneThe yarn after being cleared from spinning faults has to be wound on packagesof suitable shape, size and built. This is done at the winding zone. The windingpackages can be either in the form of cheeses (rectangular side packages) orcones (tapered side packages). However within these two types of packages, thepackage built can vary depending upon the end use of the package. Two types ofpackage builds are possible at the winding machine:(1) Precision Package Built(2) Non-Precision or Random Package Built(1) Precision Package BuiltThe precision package built can be obtained by placing coils of thread side byside parallel to one another and at a small predetermined and precise distance.In order to obtain such package built, it is necessary that the package shouldhave flanges on its sides; otherwise the package will not be stable and wouldcollapse. If the package does not have flanges, then this package built can stillbe use by giving a small taper to the package on both sides Taper Precision Wound Package Linear Traversing GuideIn order to place the successive layers of thread parallel to each other on thepackage, a to and fro movement must be given to the yarn by using lineartraversing guides. In each revolution of the machine, the traversing guide movesby a very small precise distance so that the next layer of the thread may be
103. wound parallel and close to the last layer. The distance between the twosuccessive layers of thread is called as the pitch or gain. The density of thewinding package depends upon the pitch. Minimum pitch would give themaximum dense package. The pitch can be determined and controlled by thelinear movement made by the traversing guide in each revolution.The winders that give precision built to the package are also called as spindledriven winder since drive to the package is directly obtained from a rotatingspindle.(2) Random Package BuiltIn this type of package built, the successive coils of the thread are wound at aconsiderable helix angle so that the layers cross each other to give stability tothe package. Here the pitch between the successive layers and the angle of windof each layer is considerably high. Also the packages used do not have flangeson the sides. This high pitch and high wind angle does not make the packageunstable. Coil Random Wound Package Rotary Grooved DrumThe winders that give random package built are also called as random winder.Since the random winders make use of grooved drum for winding, they are alsocalled as grooved drum winders. The package on such winding machines isdriven by the frictional contact of the rotating drum with the package. Notraversing guides are used in this case because the grooves in the drum causethe yarn to traverse on the package.Based on the type of package built given by the winding machine as mentionedabove, the winder are also classified on this basis as:(1) Precision Winders or Spindle Driven Winders(2) Random Winders or Grooved Drum WindersWhether the package is precision built or random built, following parameters ofthe package are important and can be changed according to the requirements:(i) Size and weight of the package.(ii) The compactness of the package.(iii) In case there is a taper in the package, the angle of taper is also very important and is changed for different package requirement.
104. The Type of Package DriveThe type of package built is largely dependent upon the type of driving methodused for winding. In order for the winding to take place, the package tube ismounted on the driving shaft or spindle and is driven by one of the followingmethods:(a) Positive or Direct Drive.(b) Negative or Indirect Drive.(a) Positive or Direct DriveIn positive or direct drive, the package is directly driven by the motor by meansof gears, shafts, pulleys, etc. In this type of drive, the rotary speed of thepackage remains constant through out the package build.The main disadvantage of positive drive is that as the diameter of the packageincreases, the surface speed of the yarn also increases. This causes the tensionon the yarn to increase. The variation of the tension on the yarn from start ofpackage winding to end varies; this gives variation in package build. Alsotowards the end of package winding, the increased tension may also cause theyarn to break. To avoid this with the direct drive, a PIV gear is used whichreduces the rotary speed of the package with the same proportion as that of itsincreasing diameter so that the surface speed may remain constant and uniformwinding from start till finish may be obtained.(2) Negative or Indirect DriveIn the negative or indirect drive, the package is driven by the driving roller by africtional contact. So this type of drive is also called as frictional type drive.
105. The main advantage of this type of drive is that the surface speed of the yarnwill remain constant through out the package drive. But the disadvantage is thatsince this type of drive uses frictional contact, so the yarn may get damaged.The negative drive is usually implied using a grooved drum and no lineartraversing guide is used to facilitate winding on the entire length of the packagebecause the grooves of the drum also cause the yarn to traverse through thepackage length. The negative drive is sometimes also referred as grooved drumdrive or random drive.The cotton spun yarns are mostly wound by using the grooved drum type ofdrive with a random or non-precision package built. In case of the drum drive,the drum is mounted on the shaft or spindle that directly gets its drive from themachine. Each spindle is supplied with an independent motor for its drive thatcan produce a speed of up to 1500 meters per minute. The package is mountedon a cradle which not only holds the package but also applies considerablepressure against the winding drum to avoid any slippage in the drive. The cradleis lifted as soon as the yarn breaks or the ring bobbin is emptied so that thepackage drive may be disconnected.Auto Creeling and Auto Doffing DevicesRemoving of the supply package (ring bobbin) when it is emptied and replacingit with a new full supply package (ring bobbin) is called as the process ofcreeling. On old conventional machines this process is carried out manually byhand however on the modern winders, arrangements are given thatautomatically does the creeling process. The creeling arrangement does thefollowing necessary tasks:(i) Stops the machine when the supply package exhausts.(ii) Removes the empty bobbin tube and ejects it into a special compartment.(iii) Inserts a new supply package from the creel.(iv) Performs the piecing of the thread.(v) Restarts the winding process.Similarly removing the full wound package (cone or cheese) when the requiredpackage size is obtained and replacing it with a new empty one is called as theprocess of doffing. The automatic doffing installed on the modern windersperforms the following functions:(i) Stops the machine when the required size of the package is wound.(ii) Removes the full winding package and transfers to a conveyer belt.(iii) Places an empty tube into the cradle(iv) Pieces up the yarn on the new package.(v) Restarts the winding process
106. THE ROTOR SPINNING PROCESSIn the production of short staple spun yarn, the rotor spinning technique is anexcellent modern alternate to the old classical ring spinning method due to itshigh productivity advantage over the ring spinning. The rotor spinning is not onlyhighly productive but also very cost effective at the same time. In addition toshort staple spinning, long staple rotor spinning machines have also beenmanufactured only to produce coarse yarns from long staple manmade fibres.However wool fibres because of their scaly surface, crimp and natural greasesare not possible to spin using this technique.Rotor spinning was commercially introduced in 1967. In its early years, the rotorspinning was mainly used to produce coarse low quality yarns. However withmodern developments, it is now possible to produce high quality yarns up tocounts of 40 Nc. Furthermore the rotor speed has been successfully increasedfrom early range of 40,000 rpm to 150,000 rpm. These latest developmentshave given rotor spinning technique capability of producing high quality yarns ata productivity rates of up to 10 times higher and as low as one third of the costas compared to that of ring spinning technique. The biggest limitation faced byrotor spinning is its inability to produce very fine yarns that otherwise can easilybe spun by using ring spinning. Despite of this limitation, rotor spinning is a verygood competitor of ring spinning and is capturing the market considerably incoarse yarn counts.The rotor spinning technique is quite different from the conventional ringspinning. The differences are in the following aspects:• In ring spinning, the opened and cleaned fibre mass is converted into a strand form and a yarn is created by successive drafting and twisting at various spinning stages without disturbing the linear strand form of the fibres. Whereas in rotor spinning, the strand of fibres is first separated by vigorous drafting and is then recollected and twisted in a component of the machine called as a rotor.• The feed to the rotor frame is given rarely in the form of card sliver or most commonly in the form of drawn sliver. Since rotor spinning is a true sliver to yarn conversion as compared to ring spinning where no additional roving process is required, the productivity rates are much higher; it covers less floor space and is less labour extensive.• In ring spinning systems the package formation i.e. winding and twisting is an integral part of the spinning system whereas in rotor spinning, the package winding is quite separate from drafting and twist insertion.• The rotor spinning produces fewer spinning faults like thick and thin places as compared to ring spinning, so rather than carrying additional winding and clearing process after spinning, the winding section of rotor frame directly produces suitable large packages required for subsequent processing with built-in clearers to remove spinning faults. This further makes the rotor spinning more economical and more productive.• Instead of using the classical roller drafting, the rotor frame utilizes dispersion drafting technique. The method of twist insertion is also different.
107. In rotor spinning twist is inserted by the rotation of the rotor whereas in ring spinning the rotation of the traveller around the ring inserts twist.Functions of Rotor Spinning ProcessFollowing are the important functions of the rotor spinning process:(1) Opening & Attenuation, the fibres in a sliver form are vigorously opened up into individual fibre form using opening roller having its surface covered with sharp teeth or spikes. The vigorous opening of the fibres in this way also helps to reduce the linear density of the material. The amount of reduction in the linear density depends upon the yarn count to manufacture and can be controlled by the rate of feeding and degree of opening carried out. The drafting technique used here also called as dispersion drafting is quite different from the roller drafting technique used in ring spinning.(2) Cleaning, during the opening of the fibres into individual fibre form, cleaning is carried out by removing trash particle and dust particles using trash removal devices. The cleaning at the rotor spinning is optional and is only used for more dirty cotton. It is very important that fibres reaching the rotor must be free from any trash particles or fragments because they can rapidly clog the rotor causing thick and thin places, neps and uneven compactness in the yarn.(3) Improving Evenness, back doubling is used to make an even and homogenised rotor spun yarn. The term ‘Back Doubling’ refers to opening of the fibres in individual form and recollecting them at the rotor for yarn formation. The evenness achieved by this method is far more than that achieved at the ring spinning.(4) Twisting, in order to impart strength to the yarn twist is vital. Twisting is carried out by collecting the individually opened fibres and subjecting them to high speed revolving rotor. The centrifugal forces caused because of high rotary speed of the rotor cause the fibres to get collected around the wall of the rotor in form of a yarn and with one complete rotation of the rotor, one twist is imparted.(5) Winding, the yarn produced by opening (drafting) and twisting is finally wound on finished packages. Unlike ring spinning where the package has lot of defects and also the size of the package is very limited due to ring / traveller arrangement, the winding portion of the rotor frame produces suitable bigger packages that can be directly used for next stage of processing i.e. weaving or knitting. In modern rotor machines, electronic clearing devices and automatic yarn piecing arrangements have also been provided.Working Areas of the Rotor FrameThe rotor spinning process can be divided into following areas:(1) Feeding(2) Opening & Drafting(3) Fibre Transport
108. (4) Fibre Reassembly(5) Twisting(6) WindingAn illustration showing a typical rotor spinning process is shown below:(1) Feeding ZoneThe feed to the rotor machine is either done in the form of card sliver or drawnsliver. Most commonly drawn sliver of either first or second passage is used as afeeding material to the rotor frame. The sliver is fed to the opening zone withthe help of a feed roller. The rotation of the feed roller grips the fibres andpresses is against the presser plate so that a controlled feed may be given to theopening zone of the machine.(2) Opening & Drafting Zone
109. The separation of fibres from sliver to individual form is critical for uniform yarnformation. If fibres are not delivered to the rotor with proper individualization,the resultant rotor yarn will lack orientation and uniformity. The opening of thefibres is carried out with the help of a rotating opening or combing roller whosesurface is covered with saw teeth. As the sliver is fed in the opening region, thefibres are caught by the teeth of the opening roller. Here the centrifugal forcesand the aerodynamics of the system, transports the fibres from the teeth of theopening roller to the fibre transport tube. In the fibre tube an air stream isprovided that further does the opening and ultimately deposits the fibres in therotor.As the fibres are separated from one another, the opening roller also performscleaning. Cleanest possible fibres should be fed to the rotor machine, however atsuch high degree of opening, some fine trash particles and dust will begenerated. The trash extraction unit is designed so that lighter fibres are allowedto be carried away with the air stream into the fibre transport tube while theheavier trash particles will directly fall due to their weight into the trashextraction duct.This extensive opening of the fibres results in drafting of the input sliver materialand reduces its linear density. The type of drafting employed here is called asdispersion drafting which is quite different from the roller drafting techniqueused at the ring spinning frame. Usually a draft of range of 100 to 200 is appliedduring opening.(3) Fibre TransportThe fibres opened up by the opening roller must be transferred to the rotorwithout getting disoriented. This is achieved by using a specially designedtransport tube. The fibres are transported by this tube with help of air currents.The transport tube is slightly tapered to accelerate the air currents and fibres sothat hooked surfaces caused by teeth of opening roller may be straightened outand fibres can be oriented.(4) Fibre ReassemblyThe fibres coming from the transport tube are accumulated inside the rotor.Rotor is the main component of the rotor spinning process. Rotor is just like asmall metal cup with inclined walls having a conical shape. The inclination isessential so that the fibres coming from the fibre feed tube can slide downwards.The inner surface of the rotor is called as collecting groove. The diameter of thecollecting groove also called as the rotor diameter depends upon the speed ofthe machine and fibre length. As a rule, the rotor diameter should never be lessthan 1.2 times the staple length of the fibres being processed. Collecting Groove
110. The rotor is generally made of aluminium or steel having its surface covered withdiamond particles covered in Nickel to reduce wear and increase its working life.A shaft is fixed to the rotor so that when it is rotated, the rotor will also rotate.The rotor rotates inside a stationary cover or housing with the help of a bearing.In the middle of the rotor a withdrawal tube or doffing tube with speciallydesigned mouth piece or navel is provided for the yarn to leave the rotor.As the fibres reach the rotor rotating at extreme speeds, the centrifugal forcescause the fibres to be recollected as untwisted strand of fibres. It takes manylayers of the fibres to make up a sufficient thickness of fibres necessary for yarnformation. This may happen over a period of many revolutions (approximately100). The numerous doubling of the layers of fibres provide blending called asback doubling. This back doubling makes the rotor spun yarn very even withfewer thick and thin faults as compared to ring spun yarn.(5) TwistingThe twisting occurs with the action of rotor, navel and the take-up rollers. Yarn Rotor Shaft Navel Collecting Groove Doffing TubeAs individual fibres emerge simultaneously from the fibre feed tube, they slidealong the inner wall of the rotor and are collected around the collecting groove.In this way a continual fibre ring is built up in the groove and this process iscalled as the back doubling. As the sufficient number of fibres has reassembledinside the rotor wall, further fibre feed will choke the rotor. However rotor’sspecial aero-dynamical design and due to excessive centrifugal forces acting onthe fibres, the yarn is allowed to extend from the rotational axis of the rotor toits outer surface and ultimately carries the yarn to the navel from where it canbe drawn forward with the help of a take-up rollers.Each revolution of the rotor inserts one twist in the yarn. The twist travels fromthe back of the navel to the point where the fibres leave the rotor. When thetwist in the yarn reaches the maximum level, the yarn end begins to rotate onits axis. It is necessary at this point to carry the yarn perpendicularly out of the
111. navel with the help of the take-up rollers. Mathematically the amount of twist iscalculated by the following formula: Turns per inch = Rotor Speed (rpm) / Delivery speed of yarn (“/min)However the calculated twist always comes out to be 15 to 40% lower than theactual twist imparted on the yarn. This is due to the fact the fibre slippageoccurs during the actual twist insertion.Since the yarn travels through the navel and the doffing tube with a rollingaction touching their surfaces, false twist is inserted in addition to the real twistinserted at the rotor. So the total twist inserted in the yarn is the sum of the realtwist and false twist. The false twist provides more stability to the yarn howeverduring the package winding the false twist is automatically removed and the finalyarn only has the real twist in it. The false twist does have a considerable impacton the yarn characteristics. At higher rotor speeds due to more centrifugalforces, the amount of false twist inserted during yarn formation will be more.The increase in the false twist increases the amount of wrapper fibres in the yarncausing the yarn to have more protruding fibres and a harsher look and feel.Since the yarn passes out of the navel in a rolling action touching its surface, thesurface and design of navel has a great influence on levels of false twist andultimate quality of the yarn. Based upon the type of the yarn to produce,different shapes and roughness of navels are available as shown below: Smooth navel for smooth 3-Groove navel for 4-Groove navel for non-hairy yarns low yarn hairiness low yarn bulk 8-Groove navel for 8-Groove navel for Ceramic spiral navel for low twist yarn high hairiness Low bulk & low hairinessIn general as the number of grooves increases, the hairiness of the yarn alsoincreases. Similarly rougher the surface of the navel, the yarn will have morefalse twist along with hairier, rougher and bulkier surface.
112. Just as the navel surface and design has influence on the yarn quality andhandle, the design and surface of the doffing tube also can influence the levelsof false twist and quality of the yarn.(6) WindingThe yarn formed at the rotor leaves the rotor spin box and is finally wound into afinished package. Unlike the ring spinning frame where the size of the package islimited because of the ring / traveller arrangement, bigger cross woundpackages are produced either in form of cheeses or cones. During the process ofwinding spinning faults are also removed to produce an even fault free packagesthat require no additional processes and can be directly used for weaving orknitting. Cross-Wound Package Traversing Guide Driving Drum Bow Guide Yarn Take-up RollerThe yarn produced at the rotor is continuously pulled by the pair of take-uprollers placed just after the doffing tube and ultimately winds the yarn on thepackage. The package is driven negatively by the frictional contact of the drivingdrum. To wind the yarn evenly throughout the package length, a lineartraversing guide is used. However in case a grooved driving drum is used, thislinear traversing guide is no longer used as traversing is performed by thegrooved drum itself.Winding is only possible if the surface speed of the yarn being wound on thepackage is more than that at which the yarn is delivered. This creates a tensioncalled as the winding tension. The winding tension controls the compactness ofthe package. More the winding tension, more compact and hard packages areformed and vice versa. In case the package is to be dyed, the winding tension iskept low as compared where normal weaving or knitting packages are formed.
113. For knitting yarns, waxing devices are used to apply wax to the yarn so that theyarn is lubricated to reduce yarn to metal friction in the knitting needles so thatthe wear of knitting needles may be reduced.Electronic Clearing & Automatic Piecing DevicesThe modern rotor spinning machines are also equipped with electronic clearersto remove the spinning faults and automatic piecing devices to repair the brokenends of the thread. Since the number of thick and thin places produced by theprocess of rotor spinning is far less as compared to the ring spinning, mostcommonly one piecing device is used for 10 to 12 rotors. The piecing deviceseither reciprocate in between the specified rotors or they move in an endlesscircular path around the rotors. As the piecing device finds a stopped rotor, inaddition to automatic piecing, it will also open up the spin box and will clean therotor with the help of a specially designed brush.The automatic piecer works on pneumatic principle similar to the one used inautomatic winding machines. The piecing is carried using splicing technique withthe help of air currents and air suction.Structure of Rotor YarnThe inner core of the rotor spun yarn is similar to a ring spun yarn. However theouter surface of the yarn has its unique structural build up owing to the methodof yarn formation. During the yarn formation the fibres are reassembled with inthe collecting groove of the rotor and are twisted to form a yarn. During thetwisting of fibres into a yarn, portion of fibres instead of being twisted into theinner yarn structure are wrapped around the outside of the yarn. These fibresare called as wrapper fibres or bridging fibres as shown below: (A) (B)
114. (C) (D)The wrapper fibres make the rotor spun yarn harsher and hairy in appearance.They also contribute to increased needle wear in knitting and increased wear toloom components in weaving. Fewer the wrapper fibres present in the rotoryarn, more it will resemble to the ring yarn and the better the rotor yarn will be.The formation of wrapper fibres depends upon many factors, most importantones are:(1) Rotor Speed, with increasing rotor speeds, because of the centrifugal forces both the level of false twist and the yarn rotation at the navel increases and hence more wrapper fibres are wrapped around the main core yarn.(2) Rotor Diameter, with smaller rotor diameters, the wrapper fibres are wound fewer times around the yarn core making it more hairy but less bulky (more compact) as compared to rotor yarns spun on larger rotor diameters as shown below:(3) Fibre length, longer the fibres being processed, larger rotor diameters are required otherwise the fibres will get damaged. So when larger rotor diameters are used at high speeds for longer fibres, the amount of wrapping fibres will increase.(4) Friction between fibre & rotor groove, more the fiction generated between the two, more wrapping fibres will be generated.(5) Surface of navel, rougher the surface of navel, more wrapping fibres are generated and vice versa.
115. The increase in the rotor speed is limited due to the amount of wrapper fibresgenerated. The speed of the rotor can be increased using smaller rotors becausewith smaller rotor diameter, less centrifugal forces are generated. This allows tofurther increase the rotary speed of the rotor and ultimately the productivity. Forexample, the centrifugal forces produced by a 30 mm rotor running at 120,000rpm are approximately the same as that of 36 mm rotor running at 80,000 rpm.However this is also restricted by the fibre length because for a specific fibrelength a specific rotor diameter has to be used.In general all these factors related to wrapper fibre formation must be adjustedin such a way so that the wrapper fibre formation may be minimized. Thewrapper fibres can not be entirely removed otherwise the productivity will suffera lot, however excessive wrapper fibre formation should be avoided as itdegrades the quality and appearance of the yarn.Advantages of Rotor Spinning(1) The rotor spinning produces yarn at productivity rates of 4 to 10 times as compared to the ring spinning process.(2) The cost of production of rotor spun yarn is quite low as compared to ring spun yarn and can be as low as one third.(3) Additional processes of roving and winding/clearing is eliminated. That not only makes rotor spinning operation more economical but also the capital cost of machinery and floor space requirements are reduced.(4) Due to dispersion drafting and back doubling process, rotor spinning generates fewer spinning faults like thick and thin places.(5) The rotor spinning process is the first fully automated spinning process.(6) Less energy is required to produce a yarn on rotor spinning system as compared to the ring spinning system.(7) During the fabric formation at knitting or weaving less fibres are abraded off the rotor yarn as compared to the ring spun yarn.(8) The dyeability of the rotor spun yarn is better than the ring spun yarns.Disadvantages of Rotor Spinning(1) Although many developments are carried out in rotor spinning even now rotor spinning can not produce finer yarns otherwise easily possible to produce with ring spinning(2) The presence of wrapping fibres in the rotor spun yarn gives it a harsher and hairier look.
116. (3) The rotor spun yarns have high pilling property as compared to ring spun yarn.(4) The strength of the rotor spun yarn is less than that of the ring spun yarn (about 70% of the ring spun yarn).(5) The rotor spun yarn causes more wear of knitting needles and loom components as compared to the ring spun yarn.(6) The rotor spinning process is more complicated as compared to ring spinning and the know how of operation and maintenance is less as compared to ring spinning which is widely accepted and universal form of spinning.(7) As far different varieties of yarns that can be produced, the rotor spinning system is a less flexible system as compared to ring spinning system.(8) Rotor spinning system can not be employed for woollen and worsted fibres.THE AIR JET SPINNING PROCESSThe air jet spinning technique was introduced in early 1980s as an excellentalternate to the ring spinning. The early design of such machine was capable ofproducing yarn at a production rate of about 160 meters per minute ascompared to the ring spinning frame where the productivity ranges up to 15 to20 meters per minute making it 8 to 10 times faster than the conventional ringspinning process. With new developments and better nozzle designs it is nowpossible to produce air jet spun yarns at production rates of up to 350 metresper minute making it about 20 times faster than ring spinning.The air jet spinning is not only extremely fast but also produces extremelyuniform yarns as compared to ring or rotor spinning. Furthermore the air jetspinning can produce much finer yarns as compared to the rotor spinning. Themain disadvantage of air jet spinning is that so far effective spinning is restrictedto 100% synthetic fibres or blends of synthetics with cotton. 100% pure cottoncan only be processed in combed form. However even then the yarn producedhas low strength as compared to the ring spun yarns. Another problem ofspinning with cotton fibres is dust and dirt. The air nozzle of the air jet spinningsystem is sensitive to any dirt and dust present in the fibres and createsclogging and choking problems of the nozzle. At the moment cotton air jet yarnsare only possible to spin from high quality longer, finer and cleanest fibres.Another disadvantage of the air jet spinning is its inability to spin coarse countsof yarns because of its air jet spinning technique. The general range of countsthat a air jet spinning system can produce ranges from 15 to 60 Nc. So yarncounts coarser than 15 Nc are not possible to spin using this technique.Functions of Air Jet Spinning Process(1) Drafting, the classical roller drafting technique is used for drafting under extreme controlled conditions to give a draft that ranges from 100 to 200. The older version of air jet spinning machines used to have 3 over 3 roller drafting arrangement with double apron control system. However the latest machines are based on 4 over 4 roller drafting arrangement again with the double apron system. The input material in case of processing synthetic fibres is given in form of a drawn sliver passed usually through
117. three draw frame passages. However cotton fibres must be processed in controlled conditions and is usually carried out for high quality of fibres in the combed form.(2) Twisting, the main unique feature of the air jet spinning machine is the special twist imparting technique employed. False twisting is applied to the drafted fibre material with the help of nozzles that generates powerful air pressure to fibres to convert them into a yarn.(3) Winding, the winding of the yarn takes place either in the form of a tapered packages (cones) or parallel packages (cheeses). At winding, yarn clearing and automatic piecing devices are also provided to automatically remove the spinning faults i.e. the thick and thin places and to piece the broken thread together.Typically the air jet spinning machine is divided into four distinct working regionsor zones.(1) Creel Zone(2) Draft Zone(3) Nozzle Zone(4) Winding ZoneA working illustration of a modern air jet spinning machine (Murata MJS 802) isgiven below:
118. (1) Creel ZoneThe air jet spinning machines usually have 40 to 60 spinning positions. So thecreel portion of the machine can hold these quantities of drawn sliver cans.Usually drawn sliver which has been passed through three passages of the drawframe is preferred as input material to have adequate fibre parallelizationnecessary for air jet spinning. The sliver coming from the creel portion passesover stationary creel rods usually made of plastic and is directed into thedrafting arrangement.(2) Draft Zone
119. The earlier version of air jet spinning machines, 3 over 3 roller drafting wasused. However the latest air jet machines utilizes 4 over 4 roller drafting toachieve better and higher draft distribution. Conventionally the drafting rollersare numbered from front to back. So the front rollers would be pair # 1 and theback rollers, pair # 4. The in-feed sliver is directed to the back pair of rollerswith the help of a special condenser or trumpet guide placed before it. All thetop rollers are covered with special synthetic rubber coating while the bottomrollers are steel fluted. The top rollers are pressed against the bottom rollerswith considerable nip pressure. The second pair of rollers are covered withdouble aprons to have a better control over the fibres during drafting and tosuppress the drafting waves. Both the aprons used are short. Another trumpetguide or condenser is used in between the second and third pair of rollers toavoid fibre strand being torn apart during drafting.The roller settings (spacing), cot pressure, apron height, apron spacing, apronpressure and condenser size within each draft zone can be adjusted to vary theyarn characteristics. Such a roller drafting arrangement permits drafts of 50 to200 depending upon the required yarn fineness. However drafts of above 170tend to create thin places in the yarn. The 4 over 4 drafting has three draft zones namely break or back draft zone(between 4th and 3rd rollers), intermediate or middle draft zone (between 3rd and2nd rollers) and the front or main draft zone (between 2nd and 1st rollers). Usuallybreak draft in majority of the air jet spinning machines is kept fixed at 2. Thesuitable draft in the main zone is selected and the leftover draft is given in theintermediate zone. Since the total draft is a product of all individual drafts somathematically: Total Draft = 2 x Intermediate Draft x Main DraftThe value of main draft chosen should be such that the intermediate draft maynot fall below 1.15 otherwise spinning stability will be affected.The linear density of the sliver after passing through the drafting rollers reducesconsiderably but the fibres are not separated from one another. The advantageof fibres not been individually opened up is that it is not necessary to recollectthem as in the case of rotor spinning. However the disadvantage is that no backdoubling occurs. This highly attenuated fibre strand is then passed through thespinning nozzle where false twist is imparted using power air generated by thenozzles.(3) Nozzle ZoneIn the nozzle zone sometimes one or two nozzles (varies from manufacturer tomanufacturer) are used to impart the false twist to the attenuated fibre strand toproduce a yarn. A typical two-nozzle arrangement is shown below:
120. Two nozzles (N1) and (N2) are used as depicted from the above illustration. Thesecond nozzle (N2) is actually the false twisting element. The air pressuregenerated by the nozzle is so high that an air vortex rotates the air at a rate of 1to 2 million revolutions per minute. Due to this high air vortex, false twist isinserted into the yarn that goes back to the nip of the front pair of draftingrollers. The other nozzle (N1) provides lower air flow but in opposite direction tothat generated by nozzle (N2), causing the fibres in the spinning triangle tobreak free. These separated fibres are twisted in the direction of airflowproduced by nozzle (N1). As the yarn exits the second nozzle the false twist isremoved and the core fibres become aligned with the axis of sliver. But thefibres that were separated remain twisted around the core and are called asbinding fibres. The untwisting of the core fibres cause the fibre strand to expandin size thus tightens the binding fibres. The important settings that can bealtered in the nozzle zone are:(1) Nozzles pressure.(2) Shape of nozzles used.(3) Distance between nozzle and front drafting rollers.As the pressure of nozzle (N1) is increased, the percentage of binding fibresincreases. This usually increases the yarn strength but the yarn becomesharsher. The increase in the pressure of nozzle (N2) causes the false twist toincrease and ultimately the contraction and tightening of binding fibres at theexit of nozzle (N2) increases. This causes the breakage of binding fibres andultimately the yarn hairiness increases.By changing the shape of the nozzles the air vortex generated by it changes.This helps to control the yarn characteristics like hairiness and bulk. The nozzlesare made in various designs to achieve different yarn handle and character.The distance between the nozzles and the front pair of drafting rollers controlthe evenness of the yarn. With more distance since the air pressure spreads out
121. and the twist effect of the air reduces, the evenness of the yarn produceddecreases. The spacing between the nozzle and front roller nip is also dependenton the yarn count. For coarser yarns in order to avoid choking of the nozzles,the distance is kept slightly more as compared when fine yarns are spun.(4) Winding ZoneThe yarn coming from the spinning nozzle is drawn off using a pair of take-uprollers or delivery rollers and is wound on large packages that can be directlyused in knitting or weaving. The passage of the yarn also includes an electronicclearer that helps to remove spinning faults to produce a fault free package.The package is usually driven indirectly by frictional contact of a driving drum. Atraversing guide is also used to wind the yarn on the entire length of thepackage. However the traversing guide is not used in case grooved driving drumis used. The compactness of the package produced mainly depends upon thewinding tension. A winding tension originates due to the fact that the surfacespeed of the yarn at the package is kept slightly higher than that at the deliveryroller. Greater the winding tension, more compact package can be produced andvice versa.The air jet spinning machines are either provided with automatic knotting orsplicing units to automatically piece up the broken ends of the yarns. Knottingcreates a stronger but bigger and more visible piecing whereas splicing creates asmaller, less visible but weaker joint.Structure of Air Jet YarnDue the separation and wrapping of the binding fibres around the core yarn, thestructure of the air jet yarn is flattened and wavy. The air jet yarn has centralcore made of mostly parallel fibres wrapped by the binding fibres as shownbelow:The waviness in the yarn structure is mainly because of the contraction of thefalse twist and tightening of the binding fibres as the yarn exits the nozzles. Thiswaviness makes the air jet yarn most suitable for weaving filling yarn (weft)because it can be propelled at greater speeds without breaking it. Greater thebinding fibres present in the yarn strength increases but is also makes the yarnharsher. As the binding fibres are reduced the yarn becomes softer. Unlike thewrapper fibres of the rotor yarn, the binding fibres of air jet yarn should not bereduced considerably as they contribute towards the yarn strength.Advantages of Air Jet Spinning(1) The biggest advantage of the air jet spinning is its ability of producing yarn at high rates that can go up to 20 times more than that of the ring spun yarn.
122. (2) Because of lack of twist in the air jet yarn, it gives very low pilling property in the fabric.(3) Air jet spun yarns are the most suitable yarns to be used for weaving filling yarn due to its wavy structure. This enables higher weft insertion rates on the loom during weaving.(4) Air jet yarns have high degree of evenness(5) The air jet spinning technique produces less spinning faults specially thin places.(6) The air jet spinning process like the rotor spinning and unlike the ring spinning is fully automated system.(7) Due to low levels of twist, the dye-ability of air jet yarns is much better as compared to ring spun yarn.(8) During high speed fabric formation i.e. knitting and weaving the fibre shedding off the surface of the yarn is low as compared to the ring spun yarn.(9) The process of roving and winding/clearing is not required and large fault free packages can be directly produced which is not possible at ring spinning due to limited ring/traveller arrangement.Disadvantages of Air Jet Spinning(1) Air jet spinning is mainly employed for producing synthetic and blended fibres. Cotton yarns can only be spun using this technique only in combed form under ideal conditions.(2) Air jet spinning process can produce yarn counts of range 15 to 60 Nc. Yarn counts both finer and coarser than this range is not possible to produce.(3) The lack of twist makes the air jet spun yarn 25 to 30% weaker than the ring spun yarn.(4) The presence of binding fibres in the air jet yarn makes it much harsher as compared to the ring spun yarns.(5) The fabric produced out of air jet yarns shrink more as compared to ring spun yarn because of the low twist levels.Further Reading ReferencesYarn Definitions, Classification & Yarn Properties• Eurotex – Introduction to Textiles (Volume 2) Pages 1 - 11
123. By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 1) Pages 1 - 9 By W. KleinPrinciples of Short Staple Spinning• Eurotex – Introduction to Textiles (Volume 2) Pages 13 - 18 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 1) Pages 10 - 24 By W. Klein• Short Staple Yarn Manufacturing Pages 17 - 54 By McCreight, Feil and othersThe Opening Room or Blow Room• Eurotex – Introduction to Textiles (Volume 2) Pages 21 - 27 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 2) Pages 1 - 32 By W. Klein• Short Staple Yarn Manufacturing Pages 61 - 122 By McCreight, Feil and othersThe Carding Process• Eurotex – Introduction to Textiles (Volume 2) Pages 28 - 33 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 2) Pages 33 - 58 By W. Klein• Short Staple Yarn Manufacturing Pages 123 - 178 By McCreight, Feil and othersThe Combing Process• Eurotex – Introduction to Textiles (Volume 2) Pages 44 - 49 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 3) Pages 1 - 28 By W. Klein
124. • Short Staple Yarn Manufacturing Pages 209 - 236 By McCreight, Feil and othersThe Drawing Process• Eurotex – Introduction to Textiles (Volume 2) Pages 34 - 43 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 3) Pages 29 - 40 By W. Klein• Short Staple Yarn Manufacturing Pages 179 - 208 By McCreight, Feil and othersThe Roving Process• Eurotex – Introduction to Textiles (Volume 2) Pages 50 - 54 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 3) Pages 41 - 59 By W. Klein• Short Staple Yarn Manufacturing Pages 237 - 259 By McCreight, Feil and othersThe Ring Spinning Process• Eurotex – Introduction to Textiles (Volume 2) Pages 55 - 58 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 4) Pages 1 - 46 By W. Klein• Short Staple Yarn Manufacturing Pages 259 - 301 By McCreight, Feil and othersThe Winding & Clearing Process• Short Staple Yarn Manufacturing Pages 302 - 310 By McCreight, Feil and others• Weaving: Conversion of yarn to fabric Pages 32 - 84 By P.R. Lord & M.H. Mohammaed
125. The Rotor Spinning Process• Eurotex – Introduction to Textiles (Volume 2) Pages 59 - 62 By T.Rowe, K.P. Busby and others• Textile Institute Short Staple Spinning Series (Volume 5) Pages 24 - 49 By W. Klein• Short Staple Yarn Manufacturing Pages 311 - 371 By McCreight, Feil and othersThe Air Jet Spinning Process• Textile Institute Short Staple Spinning Series (Volume 5) Pages 12 - 15 By W. Klein• Short Staple Yarn Manufacturing Pages 373 - 423 By McCreight, Feil and others